FOURT H BOOK OF
EL ARTE DE LOS METALES TREATING OF THE REDUCTION OF ALL CLASSES OF ORES BY SMELTING
CHAPTER ONE CONCERNING THE USE AND NECESSITY OF SMELTING
The method most generally used for separating Metals from the Earth and Stones with which they are begotten, in order to reduce them to their due Purity and Perfection, and the method (at the same time) most appropriate and in conformity with their N ature, is by means of Fire, in ovens, which when used for this purpose are called smelting furnaces. This was practised. in the World from the beginning of the knowledge and use of Metals, until the treatment of ores by amalgamat ion was discovered and put into practice in this Imperial Village of PotosĂ, the most famous and richest of the finds of this N ew Century and N ew W orld. And, although, as has been said in previous treatises, all the ores of Gold and Silver may be amalgamat ed, for many of them smelting is necessary, and for the very rich it is more suitable; and it is thus that its use in this Village, and in other mining Districts of the Kingdom, has never been interrupted . The base metals must necessarily be treated by fire, and by it all may be perfected. Vain will be the 185
FUNDACIĂ“N JUANELO TURRIANO
ARTE DE LOS METALES
pretensions of him who is trained in the art of treating ores, even when amalgamating Silver alone, if he does not know how to smelt and refine, at least on a small scale, as has already been explained, in order that he may know of a certainty the Grade of his ore and what he should recover.
FUNDACIĂ“N JUANELO TURRIANO
CHA PTER TWO ACES ARE THE MATERIAL FROM WHICH SMELTING FURN EON THER RKS REMA AIN MADE, AND CERT
s Ore-s melti ng furnaces are made from stones, or Adobe , work and time his and mud; and, if he does not wish to lose begin it is neces sary that the knowledge of the Smel ter-m an stones with the selection of these Mate rials. Very hard they se becau , with veinl ets are not suitab le for this work er neith crack with the heat of the Fire, and fly to pieces; clown will Lime stone serve, because it will slake and break resist lime, nor ets to powder. Soft stone s, with neith er veinl Whet fire the most ; the best of these are of the kind called stone (Sand stone ). The earth from which the mud, or Adobes, is to be made these shoul d be neith er sandy nor salty, because eithe r of for this Prope rties, at a high heat, will cause fluxing, and be must earth The s. reaso n furnaces are not built of brick etc.; etre, free from all such salts as Cap peras , Alum , Saltp there is and must be, at the same time, dense and fine. If made be may job the an abun dance of good crucible clay, ed it finish is ce very lastin g; at the least, when the furna The shoul d be plaste red on the inside with this clay. ieces or Mazacotes (Furn ace-b ottom s), which are the sole-p the which in botto m of the furnaces, and the receptacles way, melte d meta l .is tappe d, may be built in the same d groun and Earth of re mixtu thoug h sorne make them of a mixcoal (Char Charc oal in equal parts , called Carbonilla haped ture) . For rever berat ory furnaces, suitab le key-s n haste and tate facili to arder Adob es shoul d be provi ded, in their const ructio n. 187
FUNDAC IĂ“N JCANEL O TURRIA NO
CHAPTER THREE THE DIFFERENT KINDS OF FURNACES AND, FIRSTLY, THOSE IN WHICH FINELY GROUND ORES ARE ROASTED
Metallurgists have invented many furnaces of various forms for smelting and refining ores. In sorne furnaces, ores which may need it are ro asted; in others they are roasted, preparatory to amalgamation ; and in others they are smelted. Finally, in certain types the Precious Metal is separated from the Base, and in still another type the Precious Metal is refined. Ores are roasted in lumps or finely ground, and in either reverberatory or mu:ffie furnaces. The reverberatory and mu:ffie furnaces of to-day have their foundations constructed in the same manner. The floor of the Reverberator y is built up to a height of a little more than a J7ara and is of the Capacity and Size that may be required. It must be solid and perfectly level. The flame enters by a bridge located between two doors, as will be explained hereafter, and a fire-box is provided, with its necessary grate bars, for the burning of Wood and the separation of the Ashes. The roasting floor of the Mu:ffie Furnace is built on arches. The two main arches are three quarters of a J7ara wide, and a little more than a J7am high; the rest of the arches are thin and built up with narrow Adobes. The distance between these small arches should be such that Adobes made of the same strong mud, one-third of a J7ara sq u are, or larger, and three fingers in thickness, will bridge over the space from arch to arch to make a level and smooth floor. Fire is lighted under each of the large arches, all the open. ings being closed, and thus the heat is communicate d to~l FUNDACJON 188
the floor space above the small arches, so that the finely ground ore thereon is roasted. On these foundations is built the chapel or flat-arched vault; it must be flattened sufficiently to prevent excessive heat loss, but must still be roomy enough to accommodate a seated Workman to plaster it after smoothing off the floor. At the highest point of the arch, midway in the furnace, there should be left a hale or door, one quarter Vara in diameter, for charging the ground ore. On the sides there should also be left two hales in the shape of chimneys, for carrying off the smoke from the fire and the roasting ore. Furthermore, there should also be two doors, one-half Vara square at the floor line, and directly opposite each other, through which the ground ore can be rabbled and the progress of the charge watched. Through these same doors the charge is removed when finished. This is the type commonly used up to the present. Nevertheless, in accordance with my practice, much fuel and time can be saved by using sheets of iron of double the thickness of a R eal (a coin approximately one-eighth of an inch thick) and of the necessary length, instead of the usual Adobe roasting floor. In this way sorne of the arches can be dispensed with, or, by using Adobe pillars with the necessary longer or shorter supporting iron bars, they can be dispensed with entirely. In arder that the sheets may not yield under the weight of the ore, when softened by heat, they should be sustained by other pillars where the span is great. Leave a fire-door at the most convenient point, and opposite to it a chimney to carry off the smoke. This Muffie Furnace is more commodious and of easier construction if made rectangular instead of round, and one and a half times longer than it is wide. With the walls built in this proportion, all the iron bars supporting the sheets of the roasting floor will have the same length. In the middle of one end-wall, there will be left a fire..,door, as in the long roasting furnaces. In the opposite and upper end, a chimney will be provided for carrying off the smoke. FUNDACIĂ“N JCANELO TURRIANO
ARTE DE LOS METALES
A coat of mud should be applied to the lower sides of the bars and sheets, so that they will be less damaged by the heat; the upper side of the sheets should be plastered, so that neither melting Sulphur nor other things may come in contact with the iron and injure it. These furnaces are entirely open on top, thus securing
e prompt evaporation and speedy elimination of the Evil Substances the ores may contain. The surrounding walls are only half a Vara or less in height, this being sufficient to hold in the fine ore. In the arch of the Mu:ffie Furnace previously described, the Evil Substances condense and fall back on the charge in an enlivened condition, to interfere later with treatment. The Rectangular F urnace is provided FUNDACIĂ“N JUANELO TURRIANO
with doors for removing the charge with rabbles, when it is finished. A-Foundation of reverberatory roaster. B-Muffie furnace; floor built on arches. C-Fire-door; also serves for removal of ash. D-Grate bars. E-Foundation of round furnace. F-Round furnace. G-Rectangular furnace. H-Chimney.
FUXDACIĂ“N JCANELO TURRIANO
CHAPTER FOUR WHICH TREATS OF THE FURNACES FOR AND METHOD OF ROASTING LUMP ORES
Ores are roasted in lumps, either to facilitate grinding, remove interfering Evils which accompany them and to or hinder the treatment by amalgamat ion or smelting, as has been stated previously. They may be roasted in Reverberatory Furnaces, similar in every respect to those used in smelting, as will be explained a little further on. Lumps ores may also be roasted in Rectangula r Furnac~s, of a length greater than their width, provided with many small openings through which they may be fired, and the air may enter, as in those furnaces used for burning brick. Firstly, lay crosswise, on the floor, pieces of thick fire-wood (if at hand) in the form of a grill; then, on top of this, charge small wood, followed by the ore, the large pieces first, then the small, and lastly the fines. Where there is no fire-wood, Yareta and Llama dung or Cow dung may be used, together with sorne layers of grass, so that the fire will spread better. Others roast ores with fire-wood or Yareta, using a squared place (Stall) of dimerĂsions suitable to the quantity to be roasted. It is closed on three sides with earth or Adobes, having no opening; the fourth side is left open; the ore is charged on to the wood in a heap or pyramid. Water is added to the fines, to get a mixture like mud for covering the ore, leaving two or three hales for draft, however, as when burning charcoal. If the ore to be roasted is a Galena, slope the bottom so that anything which may be fused will escape from the furnace and the fire, by running out of the furnace like a slag. 192 Fill-JDACIĂ“N JUANELO TURRIANO
Ores are also roasted in large earthen Vessels, whose bottoms have many perforations; the lower part of each pot is let into another vessel containing Water, and thus the Sulphur or Pitch is recovered in the same way as already explained for the retorting of Quicksilver. In addition, ores may be roasted in the same furnace used for the cooking process of amalgamation; the method is explained in a Chapter of the Third Book, and therefore I do not repeat it here. It must be noted that if ores which contain Copperas or Alum are to be roasted, the first thing of all to do is to remove these substances by washing, as explained befare in the Second Book, dealing with amalgamation.
FUNDACIĂ“N JUANELO TURRIANO
CHAPTER FIVE ORE SMELTING FURNACES; AND, FIRSTLY, THOSE IN WHICH WOOD IS USED AS FUEL
Ores are smelted with either Wood or Charcoal. There are four modes of using these, in as many types of furnaces. When the flame of Wood alone is used, Reverberatories are employed; Wood and Charcoal together are employed in Pit furnaces. The heat of Charcoal alone is used in Muffie furnaces or Tocochimbos. And, finally, in the Castellano (Shaft) furnace, the ore passes through a bed of burning Charcoal. It is best to build the furnace in a sheltered place, so selected as to have the least possible exposure to the wind. For a Reverberatory, build up a square Adobe wall of two and a half to three Varas or less on each side, according to the size desired, and one and a quarter Varas high. Inside these walls swing a circle which shall touch the four si des; fill the vacant space in the corners with pieces of Adobe and mud. Fill the centre with good Earth, slightly dampened and well rammed, to three-quarters of the height of the walls. On this place the false bottom, made of material mentioned in Chapter Two of this Book; let it be dampened with water in such proportion that when it is squeezed in the hands it will be like a Snowball; it must not be dry enough to crumble, nor wet enough to be a mud. Throw in at one time all the lining needed, and spread all over the bottom of the furnace, in such a way that it will have the shape of a Cup or concave Fount. Ram well with wooden tampers or large stones; use large stones to smooth and shape the bottom so that it all slopes to a common point. After ramming and smoothing, this lining should have a thickness of at least four or five fingers. 194
FUNDACIĂ“N JCANELO TURRIANO
The Chapel, or Arch, is made round, like the ordinary bake oven, though not so high. On one side it has a fire-box and grate-bars for burning the wood and removing the ashes, together with a bridge through which the flame enters, in all respects like that described in Chapter Five on the treatment by cooking. In front of the fire-bridge and on the opposite side, leave sorne hales for the smoke; these may be partly closed at times (for other reasons) by Adobes, instead of being plastered up, according to practice in the smelters of the Provinces of Los Lipes and Chichas. In Turco they build up a square chimney toa height of a Vara or more above the furnace, thus carrying off the smoke with less damage to those assisting in the smelting. On the two remaining sides leave two flaring triangular doorholes, about one-quarter of a Vara to the side at the inside of the furnace, and half a Vara to the si de at the outside; in one of these doors a Bellows may be fixed when it is desired to scorify or cool off the furnace; the same equipment may be used in smaller furnaces thus arranged to refine Gold and Silver. The other door is used for watching the charge, rabbling when necessary, skimming the slag when the charge is finished, or feeding when smelting on a lead bath; lastly, it is used to tap off the Litharge in cupelling, and through this door the bottoms or sheets of Gold and Silver are removed. The roof of the furnace is not closed. A round hole is left, of sufficient size to allow a man to enter without squeezing, in arder to lay the bottom on which the smelting is done, to spread the ore, to build the cupelling bottom, or whatever else is necessary. Smelting is also done with wood in Pits. Make a round Excavation, more or less of the dimensions already given for furnaces. At the bottom, hollow out a number of moulds, so that the metal or matte will not all collect in a mass. Charge a layer of grass and straw on the bottom, follow this with the thickest of the wood, then the small wood; alternate the fu el th us in layers, until the pit is filled; FUNDACIĂ“N JCANELO TURRIANO
ARTE DE LOS METALES
a hole must always be left in the centre, from the bottom up, so that lighted Coals may be dropped to the bottom to start the fire. The ore to be smelted will be charged on the top layer of wood. If it is convenient to dig these Pits close to a steep Bluff, tunnels can be driven, to make easier the lighting of the fuel charge; at the same time the melted Ore, as it runs out, is easily handled. This method of smelting is used in Las Chichas to obtain lead from Galena; it also serves for roasting Iron ores in the Districts where lron is produced.
A-Foundation walls of the furnace. B-Furnace bottom. C-Adobe grate-bars. D-Fire-bridge. E-Furnace door. F-Fire-door. G-Door to control draft. H-Ashpit door. I-Chimney. K-Another door. L-Door in furnace roof. FUNDACIĂ“N JCANELO TURRIANO
CHAPTER SIX FURNACES FOR SMELTING WITH CHARCOAL
The furnaces in cornrnon use in three-fourt hs of the World for srnelting all sorts of Ores are called Hornos Castellanos (Spanish Furnaces) in this Kingdorn. AgrĂcola rnentions only this type for srnelting. All are alike in construction, and they differ only in that, with sorne, the rnelted Ore flows continuous ly, while in others it is tapped at intervals, as explained further on. These furnaces are built Vertical, in the shape of a rectangular pillar, a little longer than it is wide. Sorne are a J7ara in height; others, alrnost two J7aras, and sorne less, according to the size of the Bellows available and the ease or difficulty of srnelting the ore. The Tuyere, into which the Bellows pipe enters, is fixed in an opening in the furnace wall a little above the furnace bottorn. T ake note that the Tu y ere nozzle rnust not penetrate into the furnace beyond the wall, because the Slag, falling on it, would be chilled by the blast, thus plugging the Tuyere. The furnace bottorn is rnade frorn two parts of ground Charcoal and one of good Earth, well tarnped. Slope the bottorn of the front of the furnace, which will be provided with a tap-hole for carrying off the rnelted ore to a Hornilla (Fore-heart h), built clase to the furnace. So that the slag rnay run off frorn the F ore-hearth, keep it well covered and heated with Charcoal, which will be lighted by the flarne and blast frorn the tap-hole. Others build round furnaces, though they are not so good as is pretended. They can be used, however, if care is always taken to ha ve the wall a hove the Tu y ere perpendicu lar; otherwise the rnelted Ore and Slag will plug it. The natives of this Country, who have not yet gotten 197
FUNDACIĂ“N JCANELO TURRIANO
ARTE DE LOS METALES
to the point of using our Bellows, employ, for smelting, furnaces called Guayras (Wind Furnaces); the same are still used in this Imperial Village, and in many other Parts. They are like the aforesaid Castellano furnaces, but differ in having the walls perforated with many holes, through which Air enters when the wind blows, at which time alone they can smelt. From the lower side of each one of these holes there projects a piece like a small Ear, which holds lighted Charcoal, so that the entering air will be heated. They are placed on high locations where wind is usually blowing. Furnaces like the Muffie Furnace of the Silversmiths and Assayers are called Tocochimbos in this Province, and rich ore, in small quantity, is smelted in them. The Indians used them for refining only. The Muffie furnace is made in the following manner. Build a small round furnace like a Reverberat ory, but of scarcely a V ara in diameter. Let it have two doors; a small one through which can be inserted a Bellows nozzle if it is desired to hasten the work; the other opposite and large enough to take the muffie. This muffie is like the half of a big Pot split from the mouth to the bottom, and perforated with many holes to allow the entrance of heat from the burning Charcoal. There should be a space of eight to ten finger-thicknesses between the rounded pait of the Muffie (Arch) and the furnace wall, to allow room for the charcoal. The mouth of the Muffie will be set flush with the furnace wall in the large door; if, however, the Bellows is to be used, the Muffie will be left open at both ends, and will communica te with the Bellows door as well. In the top of the furnace leave a round opening, provided with a burnt clay plug, through which Charcoal is fed as needed. The bottom of the furnace is lined with Charcoal mixture or a cupelling mixture, according to the work to be done, and on it the muffie is arranged. [Apparentl y the muflies used in Barba's time were not made with bottoms.-T ranslators .] Lastly, lute in a filler-piece of well-burnt Clay between the FUNDACIĂ“N JUANELO TURRIANO
Muffie mouth and the furnace wall. A clay door will be used in the mouth of the Muffie, so that the ore can be charged, the bath can be watched or cleaned, or whatever else is necessary may be attended to.
E A-Square Castellano furnace. B-Round Castellano furnace. C-Guayra (Wind) furnace of the Indians. D- Tocochimbo, or muffie furnace. E-Large door for the muffie. F-Muffie. G--Clay door (Filler-piece?) for the muffie. H-Little door (Muffie door?). I-Plug for closing firing hole in top of furnace.
FID.'DACIĂ“N JCANELO TURRIANO
CHAPTER SEVEN FURNACES IN WHICH METALS ARE PARTED AND REFINED; ALSO SOME OTHER TYPES
T o part Copper from Silver and save both, a special type of furnace is needed. The other Base Metals are parted in precious metal refining furnaces. Build a narrow furnace bed of bricks or Adobes, higher at one end than at the other, so that it will have slope enough for all the melted ore to run out of the furnace at once through a canal like a roof-gutter. The sides of this furnace bed also slope to the centre, so that all the melted ore reaches the canal. Line the bottom with good charcoal mixture, well rammed with stones or tampers; use a knife or other instrument of iron to smooth off and give a uniform slope to the bottom and canal, so that none of the melted ore will hang back. Build up small walls of ordinary Adobes on the four sides of the furnace, to hold in the charcoal. The melted ore flows out in the canal and is recovered in a Catino or Hornilla (F ore-hearth) built at the lower end. [Barba refers to a liquating furnace, for copper-lead mattes; the method of operating is described further on.- Translators.] Gold and Silver are refined in small Reverberatories, or in Tocochimbos (Muffie furnaces) when the material is little; the only difference is that a bottom of a cupelling mixture, put in as explained further on, is used instead of Charcoal and Clay. There are other types of furnaces, which are, however, only modifications of those described. A very good furnace for smelting small quantities is called Braguetilla (Pit Furnace). Make a hole in the ground from one-third to one-quarter of a Vara in diameter, and proportionally deep; 200
. FID/DAC ION JCANELO TURR IANO
line with well-tamped charcoal mixture as m the other furnaces. The side on which the bellows is placed is left open for charging ore and charcoal. The rest of the circle is built up with Adobes, and one is placed on top as a cover ' to hold back the fire. I have always used these furnaces to refine Copper. They are very appropriate for any work that requires a violent and strong heat. To the Reverberatories there is added, on the end opposite the fire bridge, a tail-like extension, which, on account of its shape and the amount of ore it swallows, sorne call the "Dragan." I t is
not vertical like the aforesaid chimney, or a Castellano furnace, but inclined. Ore is charged into the "Dragan," and, especially when it happens to be Lead ore, there is no difficulty; it is easily melted by the fire and runs clown to the charcoal mixture bottom, where it is held back and refined if necessary, or may be tapped at once if desired. [This type of fuma ce, known as V aso, is still u sed in sornĂŠ parts of Mexico.- Translators.] A campaign in one of these furnaces will continue as long as there is ore, or as long as the furnaces and workers can stand it. Also there may be built at the aforesaid part of the Ftr.\DACIĂ“N Jl:ANELO TURRIANO
ARTE DE LOS METALES
fumace [As an extension of the laboratory.- Translators] a canal half a Vara in width, with walls on each side one third of a Vara high. This will be arranged as a furnace for parting Copper and Silver, and refining may be carried on [By liquation.- Translators] without charcoal at the same time as smelting. Fitted Adobes will be at hand for closing the top of the fumace as soon as the copper ingots [Matte cakes ?- Translators] to be parted ha ve been arranged in it. In its place this method of parting will be explained. A-Fumace for parting Silver and Copper.· E-Canal for carrying off lead-silver bullion. C-Hole in the ground. D-Adobes surrounding it. E-"Dragon." F-Copper refining canal fumace attached to reverberatory. [Liquating fu mace.- Translators.]
FUNDACIÓN JUANELO TURRIANO
CHAPTER EIGHT THE INSTRUMENTS THE SMELTER OF ORES MUST HAVE
After fire and furnaces, the instruments most needed in smelting are the Blowers. They are made in various ways and of different sizes, though the type ordinarily used is the common Blacksmith's bellows. In the Provinces of Las Chichas and Lipes, where the most smelting is done, from the beginning they have used blowers only in refining Silver, because all the smelting is done in Reverberatori es. The Castellano furnace has been less used, and for this reason less Experience in the use of big bellows, or bellows moved by water-wheels or other power, has been obtained. Nevertheless, they are in use in the famous Tin District of Colquiri in the Province of Paria, close to Oruro. In every smelter there must be a pair of Steel-yards for weighing the ore received, the ore charged, as well as the Lead, or other flux that it may be necessary to add. There must also be a Balance for weighing the Silver, and in no case must there be lacking a small and very exact Balance of the kind used for assaying the bullion bars. In the latter set of weights, the greatest weight will be less than an ounce; to it will be assigned the number twenty-four; to the second, which is one-half the weight of the first, will be given the number twelve; to the third weight, six; to the fourth, three; to the fifth, two; to the sixth, one. The seventh weight, corresponding to the half of this last, will again have the number twelve assigned to it; to the eighth, six; to the ninth, three; to the tenth, two; to the eleventh, one; and to the twelfth, the zero sign. Make these weights square and place them, according to their size, in a small box which will also hord the balance and a small pair of tweezers. T o 203
FUNDACIĂ“N JCANELO TURRIANO
ARTE DE LOS METALES
obviate a calculation for each assay, place the following table in the box. The first column gives the numerical order of the weights. The second the value in M aravedis [Units of fineness, not a coin.- Translators], as used in the assay of bullion bars, although the highest assay in use is 2380 [2400 corresponds to fine silver.- Translators]. The third column gives the corresponding value of the Silver per Quintal (100 Spanish pounds) of product assayed at the ordinary market price here of fifty Reales per M arco (Eight Spanish ounces) of taxable Silver. No account is taken of halves in anv column.
1-24 2,400 M'vedis 2-12 1,200 " 3- 6 6oo " " 4- 3 300 s- 2 200 "
7-12 8- 6 9-3 ro- 2
II- I 12- o
8 4 2
Value per Quintal Carats Grains
1,250 Pesos 625 " 312 " rs6
104 52 26 13 6 4 2
" " " " " " " " "
24 12 6 3 2 I
o o o o o
o o o o o o 2 I 1. 2
Value per Quintal
22,500 Pesos II,25o s,625 " 2,812 " 1,874 " 937 " 468 " 234 " II7 " 78 " 39 " 19
The master smelter should also have test pieces of Gold and Silver, without other alloy, which commence with pure Silver and end with pure Gold of twenty-four carats; the series rises by single points, making a total of twenty-five. He should also have a set of Copper and Silver which coromenees with pure Copper and ends with the purest of Silver. It is advantageous to have the twelve points indicating the fineness of silver and thus obtain another twenty-five test FUNDAC IÓN JCANELO TURR IANO
piece set like the gold set. Any person who has had practice in these matters can easily make them. If the smelter of ores lacks confidence in himself he may entrust the work to any ingenious Silversmith; by using the delicate balance and weights just mentioned, he will find the adjustment of the proportions easy. The first point will be of pure Silver which has been proven to be such by cupellation assay and parting with Nitric Acid, so that there is no doubt as to its fineness. [At this point the author or printer seems to have omitted the instructions for making the test piece for one carat.-Translators .] For the third point of two carats, mix twenty-two parts of silver and two of gold. Proceed in this manner to make the other test pieces increasing the weight of Gold and diminishing the Silver by twenty-fourths; thus each test piece will be of as many carats as it has parts of gold. Mark each piece with its carat number, and, in the same way, proceed to make the Copper and Silver test pieces. In addition to the foregoing, there should be the following tools: An iron ladle with a handle of the same material one Vara long, to which is fixed a wood.en handle of a Vara and a half; this is used for feeding ore into the lead bath, when necessary. A hook three finger-thicknesses in length and about one wide, with its long handle of iron and wood for cleaning out slag. A tool like a chisel-bar, two and a half V aras long and two fingers in thickness, sharpened and pointed with steel at one end and drawn to a point for a length of three finger thicknesses. A tool called Hachuela (Hatchet) with its iron and wooden handle, as shown in the sketch; its use will be described further on. Big pinchers (tongs) for seizing bullion sheets, and hammers and chisels for cleaning off earth, and cutting up the bullion pigs. T ongs for dressing the assay fires and for handling the Callanas (Scorifiers) and crucibles. A stock of these latter vessels, as well as small Cendradas (Cupels), and the moulds for making them. Tamping tools, together with smooth and round stones for repairs to furnace and cupel bottoms.
FUNDACIĂ“N JUANELO TURRIANO
ARTE DE LOS METALES
A-Steel yard. B-Large balance. C-Small balance. D-Ladle. E-Tongs. F-Punch bar. G-Hatchet. H-Set of test pieces. I-Hammer. K-Crucible. L-T weezers. M-Fu mace hook. N-Chisel.
FUNDACIĂ“ JUANELO TURRIANO
CHA PTER NINE HOW TO PREPARE ORES FOR SMELTING
The careful sortin g of ores before smelting is of the greate st impor tance, because that which melts and falls on barren mater ial is held back and canno t get down to unite with the melte d bath; it m ay at times be volatilized. If there is a lack of the necessary flux, the Silver will be so fouled and mixed with gangue that it canno t get free and will be carrie d off as the finest of particles in the slag; s this I have seen not a few times in the slags of variou smelters. Roast ing is a necessary prepa ration for the ores conta ining Sulph ur, Antim ony or Pitch, if they are to be smelted in Castellano furnaces with charcoal and blast; otherwise the violence of the fire will melt the ores before these substa nces are evapo rated, and the Silver mixed therew ith will go off in the slags. However, if they are smelted in Rever berato ry e furnaces, there is not so much dange r of loss, as the charg ances Subst Evil these time gradu ally heats up at the same are volatilized before the ore melts, thereb y inflicting less damag e. It will always be impor tant to fine-crush the ores which have to be smelted in Castellano furnaces when it can cheap ly and conve nientl y be done.. The charge is thus more easily penet rated by fire, and the collector, or other aid to smelting, which should also be crushed, will all the better combine with the charge. In order that the flame e [Blas t?-Tra nslato rs] shall not carry it off, the whole charg should be damp ened with water . AgrĂcola explains with much detail how to wash (concentra te) ores before smelting. This is done very seldom 207
FUNDACIĂ“N JUANELO TURRIAN O
in these Kingdoms, except with Tin ores and, by a few, for washing out the clays from Lead carbonate ores. In the treatment of Silver ores, this ingenious but somewhat prolix method does not compete successfully with the amalgamation machine, provided a zealous effort is made to prevent the loss of Silver in the slimy water. It will be safer, in considering the ores suitable by nature for smelting, to exclude all those which are not massive and those mixed with much gangue or other sulphide ores; these should be ground and concentrated in tubs; the slimes are saved for amalgamation treatment, while the heavy part, settled in the bottom, will be suitable for smelting.
ARTE DE LOS METALES
FUNDACIĂ“N JL:ANELO TURRIANO
CHAPTER TEN THE COLLECTOR WITH WHICH SILVER ORES ARE SMELTED
Silver is begotten in ores so accompanied by things of contrary and opposite character to its own N ature that, in smelting, unless something is added to defend and collect, it is destroyed and consumed. Let him who cares to experiment melt alone a little of the richest Ruby Silver; if he urges the fire he will scarcely recover a trace of Silver, while if he melts with Lead he will recover three-fourths of its weight as very pure and white Silver. It might also be said (and I myself incline to this belief) that E vil Substances in the ores do not cause the trouble, but that there is a lack of sorne kind of cooking or moisture necessary to bring it to perfection (otherwise it would exist as White Silver); this lack is satisfied by Lead. I am persuaded to this by what Raymond teaches in various of his writings; he solidifies Quicksilver with sorne medicines that he classes as of the lesser rank; such is the product that when it is charged on the lead bath in the cupel it is all converted to Silver; without this help of the Lead, the charge would be consumed and would disappear as smoke. These effects we should not attribute to Evil Substances in the mixture, because the material with which the Quicksilver was solidified did not carry them; we should rather attribute it to the lack of the final stage in genesis, which N ature (either from lack of Time or for sorne other Reason) could not bestow. [The preceding, referring to Raymond's statements, is characteristic of much of the alchemist's jargon quoted by Barba.- Translators.] The proof of this, the same author states, is that the substances solidified by the Philosopher's Stone do not need this aid. 209
FUNDACIĂ“N JCANELO TURRIANO
ARTE DE LOS METALES
Quicksi lver bestows absolute perfectio n upon Gold and Silver, on account of their great affinity. Be the cause what it may, experience in all parts of the World, and at all times, has shown that the smelting of Silver ores with a gangue of stone or earth can only be done advanta geously with a lead collector; this lead may either be associated with the Silver ores, or added in smelting Galena ores, refinery cupel bottoms , and lead oxide, all things which contain lead to serve as a collector. Only experience in the Art can teach one to know what collector is the most suitable for use with the ore to be smelted . The collector flux must smelt with the same difficulty, or with the same ease, as the ore; otherwise, if it does not melt or flow at the same time as the ore itself, the desired result will not be attained , and the aforesaid Inconve niences will be present in full force. The most active collector is used cupel bottoms , next Galenas or Lead ores; lying between these, and the easiest to use, is Litharge . All three collectors are used in the Castellano furnaces, but only Galenas in the Reverbe ratories; such qualities are sought in the Galenas as the characte r of the ore to be smelted demand s. It is safer to melt the very rich ores on a lead bath, in a reverbe ratory or in the muffie furnace. Ores to be smelted are mixed with things opposite in characte r to the E vil Substan ces they may contain [Sulphur, etc.- Tmnslator]. These E vil Substan ces are named, and the method of recognizing them by their Fumes is given, in the Elevent h Chapter of the Second Book. The instruct ions there written down for roasting and amalgam ation pertain more properly to smelting, and therefor e much care should be taken in following them. To avoid repetitio n they are not set down here.
FUNDACIĂ“N JCANELO TURRIANO
CHAPTER ELEVEN THE THINGS WHICH AID IN THE SMELTING OF ORES
Not only does Lead, or a substance containing Lead, serve for a collector, as shown in the last Chapter; it also helps the ores of Gold and Silver to melt and flow. Lead, or leady substances, are of no advantage with base metal ores, because in the refining they are consumed by the lead. In addition, there are various other compounds for facilitating the smelting of hard and rebellious ores, but . they are of more use in assay work than in large-scale smelting, on account of their cost; for this reason no one in all these Provinces makes use of them. That which is called "Artifical Salt" is the principal flux in the assaying of ores; it is m a de by any of the following methods: First, equal parts of argols and vinegar are boiled until the salt crystallizes out, or one pound each of Llipita, (Pearl-ash ?) or other strong ash used by dyers, quicklime, argols and melted salt are boiled with .twenty pounds of urine until a third is lost; strain, and then add one pound and five ounces of salt and eight pounds of lye; boil together in a vitrified clay pot until the salt crystallizes out. Or, charge into a vessel salt and iron which has been lying in urine; cover with urine, close well and keep for one month in hot dung; at the end of that time wash the iron with the same urine and remove from the vessel; evaporate the liquid over fire until the salt crystallizes out. Or, finally, take a brine made up with equal parts of salt, soap, argols and saltpetre, and boil until it crystallizes. In order that the saltpetre may be suitable for assaying, it is prepared by boiling to dryness in a glazed pot with lime-water; repeat this operation until the saltpetre, when tested with fire, will no longer burn. 211
FUNDACIĂ“N JCANELO TURRIANO
ARTE DE LOS METALES
Another fluxing compound is made by adding to one ounce of white, easily melted, finely ground stone, four ounces of Litharge; melt in a crucible under a muffie; pour on a stone, and it will be like Glass on cooling; grind and save until needed. . Also, equal parts of argols, common salt and prepared saltpetre, well mixed, are heated together dry in a glazed vessel until the whole mass is white; finally, mix with an equal quantity of Litharge and grind all together. In addition to those mentioned, the rust and slags of Iron, lees of Wine, Vinegar and Nitric Acid used for parting Gold and Silver, all assist in maintaining the vehemence of the smelting heat. Pyrite, the mattes obtained therefrom, glass and its skimmings, salt, iron and its filings, copperas and easily melted sand are all useful. The ore takes up these substances and they defend the metal against the fire. AgrĂcola cites other compounds in his Seventh Book, where they may be seen by anyone who so desires; nevertheless, there is but little, if any, necessity for their use, because since the introduction of amalgamation only ores easily smelted are so treated.
FUNDACIĂ“N JUANELO TURRIANO
CHAPTE R TWELV E HOW TO TEST OR ASSAY ORES BY FIRE
To him who deals with ores, it is very risky not to enjoy the Good Luck of knowing how to assay and determine with certainty the values of those which fall into his hands. This advice has already been given to those who treat ores, and here I charge all Miners that they should learn to assay; this is especially necessary for those called Cateadores (Prospectors) who are occupied in hunting and discovering new mining districts. One should not trust to the amalgamation assay, as it is very deceptive, nor should one be persuaded by the judgmen t of Sight alone. Frequent ly the ore which looks like Lead contains much Silver, and that which is thought to be Copper endoses great riches. The rocks which are rich in one District, in another District will be poor, as well as the contrary. Silver ores, which are the most sought-af ter and worked in this Kingdom, are the principal Subject of this Treatise. They and Gold ores are assayed in the following manner: If the ore is already ground, as when it is to be treated by amalgam ation, mix it well, and then grab from all parts about three or four pounds; mix this portion very well and cut out from it what will weigh the same as the maximum weight in the assay set already described as being necessary. Mix this with an equal quantity of well ground and sifted Litharge; moisten with a little water, so that the mass will hold together when squeezed in the fingers. While the assay is being prepared, heat a scorifier, or, if none is at hand, a small hole in an Adobe or in the ground, lined with good clay. Build a wall of Adobes, or stone which the fire will not crack, in order to hold in the charcoal. When the 213
FUNDACIĂ“N JCANELO TURRIANO
scorifier is well heated, that is, white-hot, place in it small lighted pieces of charcoal, and on them, in two or more lots as may be necessary, charge the assay; cover with more lighted coals and help with the blower. The Litharge will quickly melt and carry with it the Gold, Silver or Copper the ore may contain. When it is well melted, which is indicated by the slag being liquid like Oil, and when the bath is well cooked, as shown by the Lead beginning to smoke, remove the scorifier and cool. Take out the Button, and refine in a small cupel previously heated for the purpose, until it gives what is called the Vuelta (Turn) at the time all the Lead disappears; this is recognized by the drops, like Oil, which flow on the surface of the melted metal until they touch the cupel and disappear in it; when these drops disappear they are followed by different colours called Damascos by smeltermen, on account of their similarity to the colors of the Damask plum. If the Button remaining in the cupel is Gold or Silver, it will be round, upstanding and bright, like the cleanest Quicksilver; if it contains Copper or sorne other metal it will be neither upstanding nor bright. Remove the Button as soon as it has set, but before the cupel has cooled; otherwise it is not easily loosened, and the bottom will be rough. If the Button has Copper, determine the fineness with test pieces; better still, do not remove it from the cupel but add barren Lead, little by little, until the Copper is removed and the Gold and Silver alone remain. Weigh the Button, after brushing and cleaning to remove any part of the cupel which may adhere. By using the table given in Chapter Nine of this Book, the value of a Quintal (100 pounds) may be ascertained. See which of the twelve weights balances the cupel button; the number following, in the column headed "Value," is the result sought. For example, if the button is balanced by weight number Nine, or number Three of the Second Order, the corresponding figure for value is six Pesos and four Reales; this is the current value of a Quintal of Silver ore of this assay. If the
ARTE DE LOS METALES
FUNDACIÓN JCANELO TURRIANO
balancing weight is number Three in the first column, the value per Quintal will be one hundred and fifty-six Pesos and two Reales, and so on. If the balance has to be made with two, three or more weights, then the sum of their values will be the value of a Quintal; thus, if the Fifth, Tenth and Eleventh weights were used, corresponding to one hundred and four, four and two, the value of the Quintal of Silver ore would be one hundred and ten Pesos and four Reales. [The discrepancies are dueto the figures in the tables being approximations only. Examples cited include fractions of a Peso.- Tran.slators.]
FUNDACIĂ“N JUANELO TURRIANO
CHAPTER THIRTEE N SOME WARNINGS IN REGARD TO THE AFORESAID ASSAY OF ORES IN SMALL QUANTITIES
Do not be satisfied with a single Assay; make two on the same lot of ore, and if they are equal the assay may be considered correct. The aforesaid Method, suited to the needs of the Prospector, is not the method for assaying Bars by melting in crucibles under a muflle. The necessary apparatus and space are not always at hand, nor is there time to heat the furnace; this is especially true in these mining districts where many are ordinarily occupied in seeking new discoveries. In the manner I have described, whatsoever the place and time, one may make Assays and they will come out very exact. In the twenty y ears I have practised assaying in different parts, I have never been mistaken in my Assays on very valuable lots of ore. If there is a considerabl e quantity of ore to be assayed, and it is not ground but in lumps, pick out ten to twelve pounds of all classes; break it into very small pieces; mix well and cut out one or two pounds to be ground; on the latter make the aforesaid Assays. I have used none of the salts or fluxes described in Chapter â€˘Twelve of this Book. While these may be necessary occasionally, in order to make ore melt more easily, if it is ground and well mixed with the Litharge, no other flux is needed. And, even if the ore is very dry [Siliceous .Translators] the addition of another part or two of Litharge will, without fail, collect the value the ore may contain. It will be sufficient for the miner always to be provided with this flux, which is very common; not everyone knows how 216
FUNDACIĂ“N JCANELO TURRIANO
to make up the other fluxes. If the ore is exceptionally rebellious, add a little common salt, well roaste d; it will help the meltin g and clean up the slag. The litharg e obtain ed in refining Silver-copper ores is not safe to use in assaying; the copper y skimmings will contain sorne Silver. In any case, grind and sift well, and assay the litharg e by itself; if it carries any Silver, subtra ct it from the results of the ore assays. If the ore to be assayed is pure Ruby Silver, black ores (Sulphides of Silver) or tarnish ed Native Silver, do not grind it; crush to grain-like particles and charge on a Lead bath in the scorifier in the following manne r: Weigh out twice as much lead as there is ore to be assayed, and charge into a well-heated scorifier; when the lead is melted and commences to scorify, charge the ore, wrapp ed in little papers , directl y onto the lead bath, little by little; melt and refine [Cupe l.- Translator s] as directe d previously. Also, the lead used should be assayed for Silver; otherwise the results will not be exact. Deduc t whate ver amoun t is found in the lead from the assay of the ore. Take the same precau tions in assaying Bar Silver to determ ine its fineness, and carry out the task as follows: Cut out a sample from the cupel pig or bar; weigh out what corresponds to the maxim um weigh t given in the table in Chapt er Eight, or two thousa nd four hundre d Maravedis. Heat a capacious cupe! and, when ready, charge on to it a quanti ty of Lead equal to the Silver. As soon as it clears up and begins to cupe!, add the Silver. Let it cupe! until the signs cited in the past Chapt er appear ; remove the clean Button and weigh again. The numbe rs on the weigh t or weights necessary to balanc e will indica te the assay in Maravedis, according to the said Chapt er Eight. The greate st value assigned to bars is two thousa nd three hundred and eighty Maravedis. The difference between this and two thousa nd four hundre d M aravedis [Theoretical fine silver of that time.- Trans lators ] is considered to offset the volatil ization or absorp tion loss due to unduly hot cupels; FUNDACIĂ“N JCANELO TURRIANO
ARTE DE LOS METALES
very frequently the cupel ahsorbs Silver with Lead. The assay values are given in tens, and the units over each are reduced to the nearest multiple of ten; thus, in an assay which gives seventy, seventy-one, two, three or four, the value is put clown as Seventy; but if it is seventy-five, six, seven, eight or nine, the value is given as Eighty, and so on.
FUNDACIÓN JCANELO TURRIANO
CHA PTER FOU RTE EN SMALL-SCALE TESTS OR ASSAYS ON OTHER ORES
se Lead shoul d not be used in the assays of Copp er, becau er ore it will be consu med and go off as a fume. The Copp when ing; weigh after shoul d be well roaste d in a scorifier n, Butto a the fire is forced, if the ore is rich, it will give up, as show the Copp er it conta ins. On weighing, the result will vein the If ore. of al the numb er of parts of it in each Quint the ng, roasti does not give coppe r abun dantl y, then, after (Bate a), samp le shoul d be conce ntrate d with care in a Chua lighte r The pulp. on amati in the same way one tests amalg The off. ed part, or earth witho ut metal , will be wash this conce ntrate is remo ved and again heate d by fire, as often as or , times two or opera tion being carrie d out one in conta may le may be neces sary, until the Copp er the samp faciliis comes clown as a cake, or Butto n. The opera tion glass. and etre saltp tated and short ened by using may Also, after the first roast and conce ntrati on, there argols be added an equal quan tity of roaste d salt, calcined le (the and glass -skim ming s; melt all toget her in a crucib the and ier, scorif deep best thing for this work ) or in a e charg the Copp er cake will be found in the botto m. After the fire, is well melte d, do not allow it to rema in long in assay the and med, consu or the coppe r will be burn t and resul t will not be exact . If the presence of Gold or Silver is to be deter mine d, Copp er in addit ion to the indic ation s of the test pieces, the in the , Lead butto n may be purified on a scorifier with poor are mann er alrea dy described. Eleve n parts of Lead er. Copp of part neces sary to scorify and cupel one 219
FUNDACIĂ“N JCANEL O TURRIANO
ARTE DE LOS METALES
Galenas, or Lead ores, are also assayed in the aforesaid manner. Heat them without flux in a scorifier over lighted coals; if the ore is not much mixed with stone or earth, the melted Lead will easily come together in the bottom. Do not allow it to be overheated, or scorified. Cool, clean, and weigh the Button. Knowledge of the Art is necessary to avoid obtaining Crudio (Matte) which is brittle and rough; this happens when the fire has not yet consumed the Sulphur, Antimony or Pyrite mixed with ore. One may recognize the presence of Matte by the black appearance of the bath; it will not open up, and there will appear Flashes or Colours, like those occasionally seen in cupel refining, when the presence of Silver begins to be noted. Proceed with the firing until these signs are lacking, the bath clears up, and begins to scorify. An ore very difficult to melt may be mixed with Iron slag to heat the charge and facilitate the fusion; the lead will then form a Button and may be separated from the slag. If the Silver content of the Lead is to be determined, the button may be refined on a cupel, and the calculation made for the quantity of Silver obtained. Tin is assayed is the same manner as Lead, although it is best to roast, grind and wash the ore first; when the concentrate is well dried it m ay be melted. T o determine if the Tin ore carries Silver, cupel on a well-heated bath of barren Lead; the spangled scum forming on the lead in the cupel should be removed with a stick as soon as it forms, until the bath clears up. Continue the firing until the Silver appears or all the Lead is consumed. Iron ore should be heated in the strongest fire possible; roast well first, then grind, using a Loadstone to separate the iron from the rock. Collect all the material attracted by the Loadstone, mix with saltpetre, and melt into a cake. Quicksilver ores should be ground and charged into a clay vessel, like a urinal. On this place a cover, with a long nose similar to an Alembic, dipping into a vessel of cold FUNDACIĂ“N JUANELO TURRIANO
water. Heat in a small furnace, and the Quicksilver, converted to a fume, will rise, fleeing the fire, be cooled off and consolidate in the top, whence it will flow to said vessel. Quicksilver ores may also be assayed in Retorts in the same way as floured or fouled Quicksilver.
Flr.\DACIĂ“N JCANELO TURRIANO
CHAPTE R FIFTEE N
SMELTING IN REVERBERATORIES ON A LARGE SCALE
U p to these our present Times, the smelting of ores in Reverber atories has been little used, or not at all, by those treating ores; and, although Reverber atories were known in the past, they were not of the perfected type used to-day, nor were they used for smelting, but for refining only. A sufficient proof of this is that Georg Agrícola, who wrote so extensive ly on everythin g pertainin g to Metallurg y, does not mention their use for smelting. Among the methods of smelting this is the most noble, and the most appropria te for ores of Gold and Silver, especially the very rich ones, such as the black Sulphides, Ruby Silver, Chlorides, the Steel-coloured ores and impure native Silver. These ores a~e melted on a Lead bath in the following manner: On the false bottom, described in Chapter Five of this book, place another bottom or lining of the mixture there described ; this, called Carbonilla, is a mixture of two parts of ground Charco al and one of Earth; moisten and stir until it assumes the consistency already described, i.e., so that it can be squeezed in the hands like a Snowball. Charge into the furnace all the material needed for the lining; spread out and place all over the furnace bottom with the hands, in such a way that it has the shape of a bowl, or plate, the slope from all parts of the circumference to the centre of the lining being equal. Ram well with stones or large tampers; smooth and level off the lining with other small round stones or an iron tool. Close the round door in the roof at once with Adobes and mud; close the side doors also with Adobes, but not so tightly as to stop the draft and escape of the smoke. Build a wood fire and continue 222
FU'\IDACIÓN JUANELO TURRIANO
er is the to add wood as consumed, in such a way that neith the furnace flame suffocated in the furnace by an Excess, nor in this fire to undu ly cold for Lack of Fuel. Cont inue ating that mann er until the furnace is whit e-ho t inside, indic at once it is ready for smelting. Char ge the pigs of lead flame the e wher e throu gh the door opposite to the bridg enter s. tity The Lead , when melted, is called the Bath . The quan the of size the to of Lead charged will conform more or less ess. Richn furnace, the quan tity of ore to be smelted, and its pounds of The ordin ary pract ice is to charge two hund red neve rtheore; rich of ds lead for smel ting one hund red poun charged have less, at Chac apa in the province of Chichas, I to smelt into each furnace fifteen hund red pounds of lead in Lipes. six hund red poun ds of rich ore from Trini dad Hill melt at to If the furnace is hot enough, the lead commences and start s once, becomes brigh t and clear, like Quicksilver, which is to scorify. Char ge one or two ladles full of ore it up break to read y to smelt, after takin g the preca ution l amou nts finely. The ore should not be charged in such smal ld it be that the bath is only partl y covered; neith er shou work the ng prolo to heap ed up. It is a lesser inconvenience ed-up ore, by unde rchar ging the ore than to roast the heap substances. which may frequ ently conta in objectionable a sweep, like pole, Stir the bath imm ediat ely with a long kad. the so that all the particles come in conta ct with d, which Proc eed with the firing until the ore is well melte liquid. and fused ly even will be recognized by the slag being tities , quan l (Smelting is also done thus in muffies, in smal pole, and with the use of charcoal.) Char ge more Ore, work is the until way allow time to melt ; conti nue in this finished.
CHAP TER SIXT EEN CONTINUATION OF THE METHOD OF SMELTING ON A BATH, TOGETHER WITH SOME WARNINGS REGARDING IT
The richer the ore the less Slag is produced. If there is much slag produced during the smelting, let it get well heated and liquefied withou t adding any more ore; then, using the hatche t, open a very small channe l in the door, opposi te to the bellows door, throug h which the slag can flow. If anythi ng should block. the channel, remo ve it, so as to not stop the flow of slag. Have at hand sorne balls of mud and ash for plugging this skimm ing-no tch when desired; these are needed because occasionally a piece of the lining at the notch is carried away, and the sudden escape of slag may carry off sorne Lead and Silver unless the flow is checked. 路 Skim off as much slag as possible in this way; it does not matter if the bath is not entirel y cleaned of slag, because when there is only a little slag on the bath it is not injurious, but helpful and benefi dal to the next charge. Skim the bath as many times as necessary, until the work is finished. If the Lead bath is very much charged with Silver, it will not take up the Silver, in the ore which has been charged, with the same Quickness and Ease that it displays on the first charges. T o determ ine this, remo ve a small ladle sample ; cut off a piece equal to the heavie st of the assay weights; refine on a -::upel and weigh. Thus can be determined the propor tions of Silver and Lead in the bath. Unless the Lead is double the weigh t of the Silver, it will be necessary to add sorne. Make this test as many times as it may seem convenient. When the ore has all been charge d and well melted, skim 224
~ FUNDACION JCANELO TURRIANO
ces of the off as much as possible of the slag. The furna thro ugh a bar iron an Province of Chichas are tapp ed with door and terhole which commences half a Vara below the g. All the mina tes at the lowest part of the furnace linin this tapgh throu out Lead and Silver in the furnace flow ground. the hole into a sloping channel mark ed out on ded for futur e Whe n cold, the meta l is brok en up and guar flow fifty or refining. Sometimes this Rive r of Silver will l may not meta more paces. In orde r that the melted small pieces spat ter, place a quan tity of grass or straw , or m strikes the of fire-wood, at the poin t where the strea amo unt of large ground. The same thing is done with the lead prod uced in Gale na smelting campaigns. to remove, In Orur o, however, when the Bullion is read y coals are the and all the doors of the furnace are opened cool quickly pulled from the fire-box, so that the furnace will allows, the and hard en the slag. As soon as the heat off with a ed clean is furnace is opened and the britt le slag up with cut ham mer; the pig unde rnea th is then divided, chisels and saved for refining. in ladles The grea ter part of the bath may be take n out o, thus Orur at and poured into moulds to cool, as is done of Las Chichas obvi ating the losses incurred in the Province ground. The when the meta l is allowed to flow on the pigs is also grea ter part of the work of cutti ng up the obvi ated by this method. silver will Assa y a little of the lead, and the resulting bullion. the in indic ate the prop ortio n of Silver and Lead nd meth od, He, however, who empties his furnace by the seco a clip sample may dete rmin e the prop ortio n by assaying mad e on difs assay of the bath . This will be exact, while in accord; the feren t bars cooled in the earth will not be ce, will conbars which cool first, or thos e near est the furna cont ain the will off tain the mos t Silver, while thos e farth est least.
FUNDACIĂ“N JUANELO TURRIANO
CHAPTER SEVENTEEN HOW GALENA ORES ARE SMELTED IN REVERBERATORIES, EITHER ALONE, OR MIXED WITH OTHER ORES
Silver-bearing Galena ores which contain enough Lead to smelt alone without any addition or other collector, even if the Silver content is low, are profitable to their owners on account of the Economies in smelting and the Rapidity with which the Silver may be recovered. In the Province of Los Chichas this class of mineral has been very common, and although the manner of smelting explained herein is generally in use, there have been, and still are, amalgamation mills treating the oxidized ores. When the furnace bottom has been put in place the charging is done ·as follows: If there are any large pieces of ore they are broken and reduced to . the size of Walnuts ora little larger. The quantity to be smelted, frequently four or five thousand pounds, is scattered in the space between the four side doors of the furnace, in such a way that they are not blocked; this is so that the flame may enter and the draft be maintained for the exit of the smoke. A good part of the furnace bottom should also be left free from the charge, so that the melted metal · can have a place in which to collect. dry and lack the very be But if the Galena ore should necessary lead to fuse by itself and make the bath, mix it with a more leady ore in such quantity as the experience of the Master Melter may judge to be demanded, according to the greater or lesser Dryness of the ore. The black and shiny ores of Silver are also smelted in this way, by mixing with Galena ores, though experience is necessary to determine their fitness, depend1ng on the facility or difE.culty with which they melt. With eight 226
FUNDACIÓN JCANELO TURRIANO
hundred pounds of black silver ore there is ordinari ly charged three thousan d pounds of Galena ore in the following manner: Place a layer of the black Silver ore in the four parts of the furnace already mentioned, and on it a layer of the Galena ore; follow this with another layer of black Silver ore and alternat e thus until all the charge is in the furnace. It must be noted, though, that the charge should be topped off with a good quantity of Galena ore. This is not a good way to smelt oxidized ores, even though they may be rich, because the accompanying Earth (Gangue) does not allow good melting, and there is danger of the Silver being lost as shots in the slag. N evertheless, if for lack of Quicksilver, or for sorne other Reason, it is necessary to smelt, grind the oxidized ore and the Galena and mix them in the aforesaid proporti on; knead with ordinary water (though if the water happens to carry Saltpetr e it will be a help in the smelting). Make into loaves or balls, and when dry charge into the furnace, where they will be smelted with but little risk. The ores having been charged in the way indicate d, the upper door will be closed and luted; the other doors will be handled in the same way as in smelting on a bath, as previously described. Fire the furnace until the ore melts. At times it happens that the furnace bottom may not be well heated and hardene d; therefore, the charge should be frequen tly stirred with a fire-hook (rabble) to loosen any part of the charge which may be sticking. Heat the charge until the Fluidity of the slag shows that it is time to skim, that is, until the slag can be drawn out into fine threads, like T affy, after a small quantity is removed on a piece of iron or wood. Open the tap-hole with the hatchet in the manner already described, and through it will fl.ow, little by little, the more liquid and highly heated slag on top. When the slag commences to fl.ow sluggishly, plug the tap-hole and fire anew; do this two or three times. In respect to the other operatio ns, carry them out as described in the Directions for Smelting on a Bath. FUNDACIĂ“N JUANELO TURRIANO
ARTE DE LOS METALES
lt is a common thing in the smelting of the black sulphides or other coppery ores, to find a layer of Matte on top of the lead and under the slag, caused by the accompanying Pyrite and abundance of Copper; this often happens with Galenas on account of the Sulphur therein. If there is much Matte it is saved; if little, it is charged on the bath during the refining. In sorne parts bellows are used with these furnaces for forcing the fire. They are so arranged that the blast forces the flame clown upon the bath, and in every way aids greatly, because Air is the great requisite which fortifies the fire and makes it more active. Whatsoever work is carried out in a .Reverberatory furnace, one must be sure to have a clean flame; when it is dark and soots the furnace, it has no force and does not smelt. This may arise from a lack of Draft through the smoke-holes, and in this case can be remedied by opening them more, or it may happen because the ash-pit is filled to the grate-bars, preventing the entrance of air to liven and clean the fire; if this latter is the case remove the ashes, and the trouble will disappear.
FUNDACIĂ“N JUANELO TURRIANO
CHAPTER EIGHTEEN WHICH TREATS OF THE METHOD OF SMELTING IN "CASTELLANO" FURNACES
Charge the furnace with charcoal sorne hours before it is necessary to commence smelting, placing lighted coals on the bottom, or start the fire after charging, by putting lighted coals jn through the tuyeres. Help with the blast, so that all the charcoal may burn, adding more if necessary, until the furnace is white-hot. Have at hand sorne wellcrushed slag, preferably Reverberatory, on account of its fusibility; then commence the smelting in the following manner: U sing an iron bar, spread the burning charco al in such a way as to close up all channels through which the ore might fall clown to the bottom without being smelted. According to the size of the furnace, charge one or two shovels of the aforesaid finely broken slag, and on it charcoal. Blow forcibly, and keep the bellows constantly in action. The slag will melt, and the metal, if it contains any, will be released and collected in the fore-hearth at the bottom of the furnace. This fore-hearth should also be heated by filling with lighted charcoal. Alternately feed slag and charcoal until the furnace operates well, when the slag will be replaced by the ore to be smelted. Pull the slag from the fore-hearth with an iron hook, and charge pure Lead into the fore-hearth bath, if the ore being smelted should so require. The campaign is commenced by smelting Slag, in order to glaze the walls and sole of the furnace, so that the Smoothness thereof will prevent the melted metals from hanging up; thus it is easier for the metal to descend and collect in the crucible. Notwithstanding that the aforesaid 229 FUNDACIĂ“N JCANELO TURRIANO
ARTE DE LOS METALES
practice is common to all ores, there are sorne which require special treatment; this is discussed hereafter, commencing with the ores of Silver and Gold. Ores which may contain Gold and Silver and at the same time sufficient Lead to be self-fluxing, are melted by simply breaking to small pieces and charging into the furnace. If they melt too easily and form Matte in the fore-hearth, plug the furnace with a hall of clay and ground charcoal. Continue the smelting in this manner for sorne time, during which the bath will be refined. Tap the furnace, and the Lead and slag will flow into the fore-hearth. Plug the furnace again and continue in this manner until the campaign is closed. If the aforesaid facility in melting is dueto the abundance of Sulphur or Antimony, smelt them with Iron-bearing ores, such as those called Chumpis, to doctor up the charge, and both classes will the more easily yield up their contents. Should the ores be dry, or contain Orpiment, add others which are more easily fluxed and which abound in Lead, even if poor in Precious Metal. Heavy lead ores and rich oxides are best smelted on a bath in a Reverberatory ; however, should one desire to smelt them in a Castellano (Shaft) furnace, Sulphides which will yield much Lead or Litharge should be ground up and used as a collector. To one part of the well-crushed ore to be smelted, add two of the collector. Mix well with a little water, and, thus moistened, charge on to small coals or grass, and proceed as before indicated. Ores which contain much Lead and Copper, such as the black Sulphides, and copper Oxides, are also smelted with the aforesaid mix; however, before commencing the campaign it is necessary to charge sufficient poor lead into the fore-hearth to form a bath. This sucks up and drinks the greater part of the Silver which the ore carries. When the fore-hearth is full, pull out, with an iron hook, first the slag on top, and then the Copper which will be found underneath in the form of matte. Keep these separate. If the quanFUNDACIĂ“N JCANELO TURRIANO
tity of Silver and Lead in the fore-hearth is sufficient, remove. it partly or entirely by ladling into moulds. lf Ruby Silver or dull-coloured or shiny Sulphides are to be smelted in the shaft furnace (although the Reverberatory bath is the surest) grind and mix them up with water and litharge, because they are very easily smelted. Close the tap-hole at intervals, so that a bath of poor lead can accumulate to collect and cook the metal being smelted; or, construct the fore-hearth in such a way that half is inside the furnace and half outside; charge sufficient lead for the bath, and proceed as directed.
FUJ\DACIĂ“N JCANELO TURRIANO
CHAPTER NINETEEN HOW OTHER ORES ARE SMELTED IN CASTELLANO (SHAFT) FURNACES
Of the ores of Copper, there are Pacos and Negrillos. 1 call Pacos (Oxides) all green, blue, or orange-coloured ores, or any other colour whatsoever, unless they are steel-like or shiny. These latter I call Negrillos (Sulphides). Smelt the well-crushed Oxides in a furnace which has the tap-hole open all the time, and without using a lead ore as a collector. Aid the smelting by mixing in Copper Matte or Copper Sulphides, or a siliceous sandy earth, or certain white stones [Calcite.- Translators] which easily smelt. The pure Copper will settle in the fore-hearth, though at times, when there is but little depth to the bath, shot-copper may be mixed with slag. If so, grind the slag and separate the copper. Charge the rest back to the fumace and continue smelting until the slag no longer carries metal. One of the signs, in this and other cases, that the smelting is finished, is that the melted slag gives off no smell. [Of Sulphur ?Translator s.] In smelting Copper Sulphides alone, it is necessary to clase the tap-hole at intervals; otherwise, unless they are cooked in the furnace for a time, they flow forth as Matte. When the fumace is tapped into the fore-hearth, separate the matte which is on top when cooled, and return to the furnace. Ores from which Lead is obtained are smelted in smaller furnaces; otherwise, it will be consumed and disappear as smoke. The sale of the furnace and the fore-hearth are made from earth mixed with Iron Oxide. The slags from lead smelting are of the greatest help in the smelting and 232
FU:--IDACIĂ“N JCANELO TURRIANO
collecting of this metal, on account of their inherent properties. Let the tap-hole of the furnace be always kept open, and keep small coals constantly on the lead bath of the forehearth, so that it is covered and thus prevented from wasting. The furnaces can be small or large, according to the relative smelting rate of the ore handled. Litharge is very quickly smelted, and, in order to obtain all its lead, without losing anything as smoke, it is best to smelt in a small furnace, not more than twelve inches high, narrower at the bottom than at the top, and with a fore-hearth similar to other furnaces. Tin ores are smelted in furnaces smaller than those used for Silver and other ores. They are not blown so strongly with the Bellows, because the Tin leaves the rock with only a moderate fire; with a violent fire the tin is calcined and turned to ash. Let the sole of these furnaces be of Sandstone, and if the walls are the same they will last longer. Sort the ore well, and wash to remove the earth or slime. Let the charcoal also be clean, because the small stones and earth often found in it foul the charge and cause much damage. In La Plata, where Tin is smelted, when the slag has been skimmed, the entire bath is covered with ground charcoal in order to prevent loss.
FUC\DACIĂ“N JCANELO TURRIANO
CHAPTER TWENTY PRECAUTIONS CONCERNING THE FOREGOING INSTRUC.. TIONS FOR SMELTING IN SHAFT FURNACES
1: . 11
Do not charge large pieces of charcoal; if they descend to the tuyere they cut off the blast, and higher up they are likely to clog. The smaller pieces will then burn out, and ore will reach the crucible unmelted. Therefore, break up the larger pieces. Even with this precaution, it is well, before charging the ore, to poke down the charge frequently with an iron bar, thrusting it in from the top two or three times in order to fill up all the holes. T ake much care that the mouth of the tuy ere, whence issues the Blast, be not plugged with the slag which may fall on it. When this happens the fire will lack force; the descending ore will not be melted; it will heap up and harden in the fire, and nothing will be accomplished until this is remedied. It may even be necessary at times to stop the work and remove the disturbance with a bar. Therefore, it is well to observe frequently if slag is cooling on the tuyere nose; and, if so, remove with an iron scraper. To prevent the slag accumulating on the tuyere, it is well to charge the ore in the centre of the furnace, and more to the side opposite the tuyere. If the furnace should happen to be plugged (as it is said to be when the ore heaps up and hardens on the sole), clean out as much ore as possible through the tuyere-hole, using an iron bar. Stop charging ore, and in its place add slag, which, on melting, will moisten and soften the hardened (frozen) charge. Thus the charge will melt again, and the furnace will clean up, allowing the campaign to be continued. On the side of the furnace opposite the tuyere, and~ FUNDACION . 234
little higher than the sole, I have been accustomed to leave a round hole, through which the hand could be inserted. This is ordinarily closed with a clay plug; but when the furnace becomes frozen I take out the plug and thus clean the furnace. This is better than cleaning it through the tuyere. The charcoal on top of the furnace should be sprinkled frequently with water, in the same way that Blacksmiths do in their forges. Not only does this serve to hold back the fire; it also causes the condensation of the finer part of the metal volatilized by the flame, which otherwise would be lost. And it is for this reason that, in sorne Parts, tall and capacious chimneys are constructed over the furnaces; the Silver carried up by the violence of the flame sticks to the chimney walls, and after a time can be removed to advantage. This method of smelting the abundant and very rich Black Silver and Ruby Silver ores in shaft furnaces with high chimneys has been used in the rich mining District of Porco since the discovery of this Country. Many times have I been in the smelting plants there, because the road from this Royal Village of PotosĂ to the Province of Los Lipes (where I resided seven years), passes through it. I know that a considerable recovery was made from the old chimneys. When the task is about over, but before stopping, charge sorne litharge. This, on melting, will carry with it any Gold or Silver which may be held back in the charcoal or stuck to the furnace walls. T o clean out the other metals, finish up with a slag charge. As the fuel leve! drops, and before the furnace cools, bar the walls free from Zinc and other crusts, using an iron bar with a chisel point three or four fingers wide.
FUNDACIĂ“N JCANELO TURRIANO
~CHAPTER TWENTY-ONE THE METHOD OF SMELTING IRON ORE
lli lu 1
The resistance of Iron ores to fire is so much greater than that of other ores that it has obliged those who occupy themselves in the treatment thereof to use greater violence (of flame) and force to reduce them and put them in condition for human use, for which they are more necessary than Gold or Silver. I have never smelted iron ores, and ordinarily I should not care to treat of this subject without considerable experimenting. This is the sole exception. Considering that in these Kingdoms there is an abundance of iron ores, and that Science may be needed in their treatment, I herewith set forth the method used (as I am informed by practica! persons) in a part of the world (Spain) no less wellknown for the Abundance of this most necessary Metal than for the Fame of the Nobility and Valour of its inhabitants. The chunks, or large pieces, of iron ore are broken clown to pieces the size of nuts or apples, so that the fire may the more easily penetrate the charge. Make a pit like unto that described in Chapter Five of this Book; arrange the wood and charcoal (as described) and on this mix and heap up the iron ore. Set fire to the charge, and, when half-melted, cool the furnace and remove the slag-like mass. Charge this mass into a furnace three feet high, and more than three feet square; line this with brasque to leave a crucible sixteen inches in diameter and eleven inches deep, more or less, according to the quantity to be smelted. Fill this chamber with charcoal; charge the ore on top, then more charcoal, followed by ore on top, thus forming a heap. Blow the fire very strongly with large bellows worked by water236
Flf;'\DACION JCANELO TURRIANO
wheels. Take care in charging that the ore is placed on the side of the furnace opposite to the tuyere in arder not to stop the blast. Continue until the ore is softened and forms one big cake; then remove the slag through the opening provided. When the smelting is finished and the furnace has cooled, pull out the cake with a pair of tongs. Knock off the adhering slag, and cut up with chisels. Heat these pieces again, and, with a great hammer moved by water, forge them into bars or sheets. Georg AgrĂcola says to grind the iron ore very fine, mix with Quicklime, and then smelt in the furnace described, without the preliminary treatment in the pit furnace. N evertheless, the method [Most ?- Translators] used is that referred to above.
fl)),l)ACIĂ“N JCANELO TURRIANO
CHAPTER TWENTY -TWO THE METHOD OF OBTAINING QUICKSILVER
li 1\ i
At no time, nor in any part of the World, has there been such frequent use of Quicksilver as in this present Century and in this Province of the Indies. This metal is needed to amalgamat e the Silver in the treasures of the rich Hill of this Village of PotosĂ, the most famous in the World; nor is this most fertile land lacking in its ore. Quicksilver is obtained in various ways, but all make use of the same principie, to wit, the ease with which the metal is converted by fire into a vapour, which, thereafter coming into contact with a cooling body, condenses and returns to its proper form, as we shall see. Bury many large pots in the earth, close together, in the form of a square. Endose this square with a low wall of Adobes to keep in the burning fire-wood. Have other pots, of the shape of chamber-po ts, wider at the bottom than the top. Fill them with well-broken quicksilver ore, and on the ore place a cover of pottery, copper or iron, which has many small perforation s. Invert these pots and place in the mouth of the large pots sunk in the ground. Lute and fire from the top. The quicksilver vapour will condense in the bottom of the large pots from which it is removed later. Quicksilver may also be obtained by retorting the ore in ' furnaces of the type used in aH mining districts of this Kingdom for roasting slimes. They are arched furnaces, of greater length than width, perforated on the top and sides with large round holes in which to place the vessels of clay called retorts. The ground ore is charged into the retorts and covered with two finger-thicknesses of well-tampe d ash. These vessels are covered with others called hoods, the joint being well clayed. Heat with a long fl.ame through i J . FUNDACION 238
end of the furnace; locate a door at the top of the furnace and at the opposite end, through which the smoke can escape. The Quicksilver willlodge in the top of the hoods, where it can be recovered. Should there be much Quicksilver, what falls back u pon the ashes can be recovered by washing the ash. The use of glazed stills (retorts) on iron bases, such as are used for retorting amalgam, is also an excellent method. In using all these methods, the Workers must always be on the windward side, on account of the great danger from the Fumes should they penetrate the vessels, or escape from a .broken one. F or this reason, and on account of their greater durability, it is best to use hoods of iron or beaten copper.
A-The square in which the pots are buried. B-Pots. C-Chamber-pot (Hood). D-Perforated plate. E-Retort. F - Hood. G- Flame furnace. H - Fire door. I-Chimney. K-Iron vessel. L-Condenser head. FlF.\'DACIĂ“N JCANELO TURRIANO
FUNDACIÓN JUANELO TURRIANO
FIFTH BOOK OF
EL ARTE DE LOS METALES IN WHICH IS DESCRIBED THE METHOD OF REFINING AND PARTING METALS
CHAPTER ONE THE METHOD FOR MAKING THE CUPELLING BOTTOMS FOR REFINING GOLD AND SILVER
The Gold and Silver issue from the furnace accompanied by a large amount of Lead (as will have been noted under the description of smelting) and also, at times, accompanied by other metals; and it is necessary that all these should be removed in arder to leave the Gold and Silver with the desired fineness. With the aid of Lead alone, the other base metals are consumed and wasted; if there is not sufficient Lead to carry out the following directions, the alternative will be discussed la ter. T o refine the Lead, it is necessary to prepare, in the following manner, what is called the cupelling bottom. First, have to hand a quantity of wood-ashany kind so long as it is free from earth, straw, or fine charcoal. It can be prepared by throwing the ashes into a tub of water and stirring well; on allowing to rest for a short time, the light substances will cometo the top and can then be skimmed; the earth and ~mall stones will settle to the bottom. Pour off the turbid water carrying the ash, and allow to settle entirely; then pour off the clear water and dry. The best ash, however, is that burned from Eones, a~ 241
FUNDACIĂ“N JliANELO TURRIANO
ARTE DE LOS METALES
it is very dry; not always, though , is there to hand the necessary quanti ty of bones and facilities to prepar e it. For this reason, the ordina ry practic e among smelte rmen is to use the ash of Yareta (a low-growing Bolivian plant, genera lly used for fuel) or Cordones. The ash of Molle (a small Bolivian tree) or any other evergreen tree or bush is also good. Burn the materi al with care, in sorne clean place where the ashes will not be mixed with earth, and sift well to remove any part which may not be burnt to ash. Sorne mix with the ashes a portio n of ground brick, so that the bottom will take up less lead and produc e more litharg e. I found a kind of white earth in Oruro, on the hill called Tetilla , which saved me the troubl e of collecting and prepar ing ashes, because from it I was able to make most excellent cupelling bottom s which absorbed lead as well as those considered the best. Charg e into the furnaces one or two sacks full of ashes, according to the size of the furnace and the quanti ty to be refined; have the floor of the furnac e clean and ramme d hard; better still, mix on a blanke t, throw on water, and knead with the hands until all the mass is equall y moistened, and, as has been described before, until a handfu l can be compressed Iike a snowball. Clean and dampe n the furnac e bottom on which the cupelling bottom is to be placed. The furnace, as said before, should be a Rever berato ry. Charg e aii the ash at one time throug h the round door in the top of the furnac e; and let a man enter throug h the same door in order to place and shape the mass in such a way that there is room for all the lead to be refined. Tamp weii, first with the hands, and then, standi ng uprigh t, with the feet; follow this by tampi ng with stones and mauls as much as possible. Leve! off and smoot h, so that, as the charge lowers, none of the lead carryin g the gold or silver wiii be caugh t and held back. The deepest part of the bottom is inclined toward s the door, placed opposi te the bellows, in order that the litharg e skimm ed there will have the least distan ce to travel. This wiii be explained farthe r on. If calcined or ordina ry salt is dissolved in the 1
FUNDACIĂ“N JCANELO TURRIANO
water used in making up the bottom, it will be denser and stronger. What are called Cupels are only small cupelling bottoms in which assays are refined. They are made in round moulds of iron or brass, greater in diameter at the bottom than at the top, shaped like a Marco (eight ounce) weight, and without a bottom, so that the cupel can be easily removed froni the mould. Place the mould on a :flat, hard stone, and fill with bone-ash, prepared as already described. Press first with the hands, then with the other part of the brass mould, having the shape of a pestle. In this way the cupel is given the necessary Concavity. Tamp the cupel with blows from a mallet or hammer, which should be ready to hand for this purpose. Remove the cupel and lay aside; the older and dryer the better they are.
A-The cupelling bottom. B-Litharge notch. C-Cupel moulds. D & E-Cupel mould. F-Mallet for tamping cupels. G-Flat stone on which cupels are tamped.
FUNDACIĂ“N JUANELO TURRIANO
CHAPTER TWO HOW GOLD AND SILVER BULLION IS REFINED
When the cupelling bottom has been finished, close and lute the doors in the same way as when smelting ore. Heat the furnace well. If a crack should appear it can be remedied in this way; make a Sludge of ashes and water; tie a rag to a pole or furnace bar; wet this rag well in the Sludge and apply to the cracks; it will do no harm to apply to all the bottom. When the furnace is well heated, as is indicated by its being white-hot, the cakes, sheets or pieces of goldor silver-bearing Lead are charged through the door opposite the fire-box, and heaped up on one another. The Lead will melt and flow clown into the concavity of the bottom, and commence at once to cupel. When the entire lot to be refined is melted, clase the charging door. After the charge is well melted, if there is a quantity of slag, remove it, in the manner already explained under smelting. If but little, charge sorne charcoal on the bath, stir with a wooden rabble, so as to collect the slag in one mass, and then pull out with an iron rake. The bath now being clean, it will give off much smoke, which the bellows blast will force out of the furnace. The Lead continues to be consumed because the bottom takes up part and a part is converted into Greta, as Litharge is called. Litharge is like grease or oil, and is easily recognized by the difference between it and the bath on which it swims. The bellows blast pushes the Litharge towards the door on the opposite side, and when a sufficient quantity has collected a very small notch is carefully opened with a hatchet, in arder to tap it out. As the level of the lead bath lowers, this notch is gradually deepened. If there is much Copper in the mass being refined (by 244 FUXDAC IĂ“N JCANELO TURRIANO
reason of its presence in the ore smelted) a grease-like scum will appear on the surface, although it will be of a darker colour than the Litharge. Put it to one side, because it frequently carries with it much Silver. The smelters of Oruro always threw away this material until I went there and bought up these Wastes, or Slags, for a small sum and recovered sorne tho~sands of Pesos in Silver therefrom. To-da y, however, from m y example, they know how to recover everything. Let there always be two well-heated pieces of the bottom mixture alongside of the litharge notch, in order to plug it, should any of the rich Lead start to flow off with the Litharge. This condition can be easily recognized by any one, even if inexperienced, because the Lead looks like Quicksilver, while the Litharge is Reddish in colour. The quantity of Litharge produced depends upon the violence of the Fire employed for the work. An excessively violent fire will not only prevent the Litharge from consolidating; it will even melt it and turn again to lead what has already been created. This Warning will suffice for the inexperienced, so that they may judge for themselves the heat necessary to maintain. The Lead finally cupels off, and, as the saying is, there comes the turn to Gold or Silver. The mass becomes covered all over with a coloured film in which there no longer can be seen the drops of Litharge that previously swam on the bath. Cease to add wood, as the heat in the furnace will cause this film to clear up, and then turn to Blue and Rainbow colours, and finally to become clear like Quicksilver, just before the sheet solidifies. Before it grows cold, pry it loose from the bottom, using the wide point of an iron poker or bar. To do this, anr! to cool off the furnace more quickly, open the doors. Work the sheet toward the furnace door with iron bars, and finally remove it from the furnace with a pair of large tongs. Refining can also be done in Muffies in the same way, but on smaller quantities. FU>:DACIĂ“N JCANELO TURRIANO
CHAPTER THREE WARNINGS IN REGARD TO THE INSTRUCTIONS FOR REFINING GOLD AND SILVER
If, when the bath and furnace are well heated, the bath, instead of clearing up, remains dark and crinkles, it is a sign that it contains Tin, and it is useless to wait for it to be cleaned up by the force of the fire. Remove the scum with a long pole, and continue to do so as many times as necessary until the bath clears up. This is the sole Remedy. When the bath clears up proceed with the refining as directed. Gold and Silver, either alone or together, show by the play of colours already described, that they have been refined. When they are mixed, the proportion of Gold cannot be determined until the sheet is removed from the cupel, sampled, and parted with Nitric Acid, as will be described further on. If the sheet finished with sorne Copper in it, or was not well refined, this fact will be easily manifested even to the half-experienced. The · bath will not clear up after the coloured film appears, nor will it become mobile and clear; on the contrary, it will become darker, and sometimes it will be covered, on cooling, with eruptions. This latter occurrence is also frequently observed after a sheet of bullion . has set, when sorne of the litharge on the sides of the cupel is reduced to lead again. Add more lead, liven the fire, and proceed as before as many times as necessary, until the play of colour shows that the bullion is duly refined. If the refined sheet of bullion should be unusually large, it will be necessary to tear out a part of the furnace at the front door in order to remove it. However, to obviate this drudgery, it will be best to remove part of the bullion as 246 FUNDACIÓN JUANELO TURRIANO
balls in the following manner: Take the steel-pointed bar already described; wet, and insert to a depth of two or three finger-thicknesses in the bullion, immediately after the play of colours has ceased, but before it has set. Sorne bullion will stick; remove the bar at once and cool in water; again insert in the bullion, and repeat this operation until a hall of the desired size is obtained. Strike the balls with a hammer and they can be easily loosened from the bar. Continue this for the desired number of balls. Much work and trouble is obviated in this way when rich ores are refined on a large scale. In this I have had more than ordinary experience in the past years in the Chacapa refining furnaces at Las Chichas. With all the bullion sheets (and they were nota few) obtained from the ores ofTrinidad Hill, Los Lipes, it was necessary to open the furnaces. The work was intolerable, not only on account of the excessive Heat, but also on account of the great Weight, as one sheet of fine Silver weighed two hundred and eighty-four pounds, while five others were only a little less. The show which I made with these enormous pieces of precious metal was not a little counterbalanced by the work it cost to get them out of the furnace, pack them to this Royal Village, and cut them up in order to make bars. Since then I have used the better practice of taking out most of the silver as balls; this is also the practice in the Oruro smelter. A cupel bottom may serve for two or three refinings, if well made with a good depth of ash, and if it has not absorbed too much lead. Remove the bottom when convenient. The part which is hard, like a rock, on account of the absorbed lead, is called M olibdena, or Cendrada, by smeltermen. Place it to one side, and use it as a collector in smelting. Sift and save the rest of the ashes, which will be the best (obtainable) for other cupel bottoms. If during the refining the heat rises to such a degree as to make the bottom and the bath the same colour, Silver will be lost. On account of the great heat it becomes unmanageable, and the cupel bottom becomes spongy and FID:DACIĂ“N JuANELO TURRIANO
ARTE DE LOS METALES
sucks into it the Silver with the Lead; therefore the edge of the cupel bottom should always be darker than the bath. The pieces of M olibdena, Cendrada, or lead-saturated cupel botom, when they are yellow inside like litharge, contain only Lead. If blackish, the bottom contains sorne absorbed Silver. Assay to determine the amount, and save (if justified).
FUNDACIĂ“N JUANELO TURRIANO
CHAPTER FOUR THE REFINING OF OTHER METALS
The base metals do not always come out of the furnace with the perfection they should have. Lead and Tin frequently come out rough and brittle on account of admixture with Mattes or · other impurities. These impurities may be removed by placing the bullion sheets or pigs on wood or lighted charcoal on a slightly sloping ground, so that, when melted, the pure Metal will run off and leave the impurities behind in the ash. The pure metal can at once be moulded into appropriate forms. The refining of Copper is even more necessary on account of its more general use, and because it cannot be beaten out if it does not possess the perfection due to it. Copper in the form of matte will break like glass; in sorne parts of Spain it is called Confrustaño. This is a mixture of Lead and Copper with Sulphur and other impurities, either created together in the mine or melted together in the furnace. Sorne persons roast the pigs frequently, and afterwards, in smelting with a strong fire, melt and purify until all the lead and other foreign substances are removed and the copper becomes refined. I, however, in refining many hundred-weight of this class of material in Oruro, eliminated the repeated roasting of the pigs, and at the same time recovered the contained Silver. Build a furnace of the type which I ha ve elsewhere called the Braguetilla [Pit furnace.- Translators]. Fill with charcoal, light, and blow with the bellows until well heated. Charge pieces of the copper (or copper lead ?) matte. These will quickly melt with the violent heat, and a great part of the impurities will be consumed, while the metal will flow down through the lighted coals. 24Q
ARTE DE LOS METALES
Add more matte and charcoa l as necessary, and so proceed until the fore-he arth is full. Pull off the slag with a rabble. Contin ue the blast until all the matte is cooked and reduced to a clear bath which contain s nothing but Lead, Copper and sorne Silver. Remov e a spoon sample and assay; if it contain s considerab le Silver, and there is not sufficient lead to part, add it in the proport ions indicat ed further on. Allow the bullion to cool and lift out of the fore-he arth. If the Silver does not justify parting , and there is very little lead, proceed with the firing until the latter is all consumed and the bath turns to fine copper. T o determ ine if the Copper has the desired fineness, thrust an iron bar into the bath; then remove it, with the copper sticking to it, and cool in water. If the copper adherin g to the bar is clean and lustrou s, like brass, it is sufficiently refined. If not, proceed (with the blast ?) until the sample gives the desired Colour. Should there be much Lead, it is best to let the bullion cool in the fore-he arth, though it may be removed and cast in pigs for further treatm ent, as will be shown later, in order to recover both Copper and Silver. In burning off much Lead, a considerable part of the Copper will also be lost. These pigs of mixed Copper and Lead, with or withou t Silver, are spongy, like pumice stone. Roast them well, and then, with a chisel-pointed hamme r, chip off the ash-like cap, which is Copper. This cap also carries sorne Lead and Silver. When cleaned, refine in the furnace as already described. Iron may also be said to underg o a refining process when Steel is made from it. The process is thus described: Make a little round furnace, eleven inches or a little more in diamet er, and eight inches deep. Line it with ordinar y mixtur e of two parts of ground charcoa l and one of mud or clay, well ramme d. Let the sides of the furnace be of stones which do not melt nor splinte r in the fire, or of half Adobes, in order to hold in the charcoa l and pieces of iron charged on top. Fill with charcoal, light and blow well with the bellows, so placed that the nozzle reaches to the middle of ' ~~ ~ JUANELO TURRIANO
the furnace. Throw in at once sorne small pieces of iron ore mixed with that class of stone which will easily melt. · (Calcite?) Blow strongly until all is liquid, like water. Then place two or three thick pieces of sheet or bar iron in the furnace and leave for five or six hours until well softened. Remove and draw out by forging on the anvil. While the iron is still hot, quench in cold water If, on breaking, the iron is white and evenly grained at the centre, it has been converted to Steel. If not, repeat the operation. When duly refined, draw out in the form of square bars, such as those ordinarily brought to us. Quicksilver is purified by washing with vinegar and salt until the washings are no longer black. Then squeeze through buckskin, or wetted close-woven linen, or retort in the usual way. All the quicksilver caught in the upper vessel is pure, and whatsoever impurity it may have contained will remain in the bottom of the vessel.
FUNDACIÓN JCANELO TURRIANO
CHA PTE R FIVE HOW SILVER IS PARTED FROM COPPER, AND BOTH RECOVERED
If considerable Copp er is mixed with Silver, it will be nece ssary to part them , not only to recover the Copp er, but also in orde r to obvi ate the excessive cons umpt ion of lead necessary for scorifying in orde r to recover the Silver. In scorifying off one hund red weig ht of copper, there are necessary at least eleven of lead. In the following meth od, altho ugh lead is used, but little is lost. Melt silver-bearing copp er bullion with lead, in the prop ortio n of three pounds of lead to one of copp er. Cast into moulds of the desired size, altho ugh I have always made the pigs of a hund red pounds, or a little more , in orde r to mana ge well. Place the pigs on edge in the appr opria te furnace, described in Chap ter Seven of Book Four . Let the pigs be placed on squa re iron bars, or on pieces of bricks, three finger-thicknesses high, and on each side of the cana l which runs throu gh the centr e of the furnace, so that they at no poin t touch the botto m or sides. Char ge what the furnace will hold, leaving a space of five or six fingerthicknesses between the pigs, to be filled with charcoal. Cove r all the pigs with charcoal, and light ; in a short time, as the heat increases, the lead will begin to liqua te, carry ing with it the silver. The copp er will not be melted. The leadsilver bullion will flow throu gh the canal into the forehear th, from which it can be ladled into moulds to be=refined later , as alrea dy described. The cupel botto m can be utilized, as before state d, on acco unt of the lead conta ined as litharge. A little copp er will also liqua te with the lead, but it will chill near the tap-h ole where the heat is less. 252
l!!l:!ru RRIAN O
These chilled pieces are called "Spines" by refiners, and it is necessary to pry them out frequently, in order to keep the lead channel open. If any of the pigs should start to melt, pull the coals away; if there are any that do not liquate freely, apply more heat to them. If desired, copper and silver may be parted in the Reverberatory furnaces already described, and used frequently by me. Arrange the pigs lengthwise in the furnace, on iron bars and pieces of brick, in such a way that an open passage is left in the middle of the fumace for its fulllength. Roof the furnace with adobes and mud, leaving a smoke hole at the end (opposite the fire-door). When the lead ceases to flow, it is a sign that the pigs are liquated. In order to prevent their melting, take off the adobes and let the pigs cool. If the copper carries much Silver, it cannot all be removed the first time with the lead. Assay the liquated copper pigs, and if they contain much Silver, melt with lead and liquate repeatedly until all the Silver is recovered. Very little Silver will remain in the chilled material at the tap-hole, so it can be remelted as convenient. Although the pigs (for refining) can be made in small scorifying furnaces, it is best to use Shaft furnaces in the following way: Have the furnace well heated, then charge in the copper; as soon as it begins to flow into the forehearth add the corresponding amount of lead, and continue to alternate these with fuel. Ladle the mixed metals into moulds for refining later. If desired, Litharge may be used, without being first reduced to metallic Lead. It should be noted, however, that one hundred and thirty pounds of litharge are ordinarily produced from a hundred pounds of lead. The copper in the liquated pigs can be refined in the manner already described.
FlT.\'DACIĂ“N JCANELO TURRIANO
CHAPTE R SIX HOW GOLD MUST BE PARTED FROM COPPER
. Although there are different methods of parting Gold from Copper, all depend on the resistance of Gold to Sulphur and other substance s which easily alter and almost destroy copper. Hence, if gold-bearing copper is melted with Sulphur, or if Sulphur is well stirred into melted Copper, an earth-like mass will result. Again, thin sheets or granulate d copper may be heated in clay pots with ground sulphur until the sulphur penetrate s all the copper and makes it so brittle that it can easily be ground. If Quicksilver is ground into this material in the ordinary way, it will recover the gold. There is another way to part Gold from Copper, utilizing Heat and the reaction derived from the salt (Mixture) called "Artificio sa" (the cunning salt). It is made with equal parts of Copperas, Saltpetre , Alum and crude Sulphur, one pound of each, together with half a pound of sal-ammoniac. Grind the foregoing well and boil with one part of fullers' earth, one of quicksilver and four of common ashes, until reduced to dryness. Grind the residue and mix with one pound of ground litharge. T o each pound of copper containin g Gold, add in the crucible, little by little, one and a half ounces of this mixture, stirring it in well with an iron wire. Allow the crucible to cool; break it, and the Gold will be found as a little button in the bottom; the copper will be on top of it in the form of matte. Reduce the matte to copper in the way already described. It will be easy for anyone who understan ds the Principies to find other ways. Sulphur, mixed with a little Lead, · is all that is needed to alter the copper without detrimen t ·t o the Gold, and therefore I am excused from writing about 254
FU)JDACIÓN JCANELO TURRIANO
other Methods, as the foregoing are not only sufficient, but ~ are also best and most generally in use. Sorne writers claim that Gold can be liquated from Copper by adding Lead, as already described in the liquation of silver and lead from copper in the last Chapter. I do not believe that they have ever tried it, having always doubted this on account of the Difficulty with which gold melts. The reason that silver can be liquated from copper with the aid of lead, is that both the lead and silver melt at a much lower heat than the copper. This is not true of gold; experiments which I have made confirm this statement. If it is desired to remove gold from gilded copper, it may be done by heating the piece to Redness and quenching in cold water; the gold may then be removed by rubbing with a wire brush.
FlJ.'\DACIĂ“N JCANELO TURRIANO
CHAPTER SEVEN THE NITRIC ACID WITH WHICH GOLD IS PARTED FROM SILVER
Gold which is e~ther artifically or naturally mixed with Silver may be parted by using Nitric Acid, which is of an admirable activity, and one of the most curious things in human experience. A knowledge of it and its use is very necessary in this Kingdom in the treatment and parting of Silver, very frequently accompanied by Gold. In a matter so important it does not do to trust to the Sight, which does not allow the mixture of these precious metals to be detected, unless the proportion of the gold is considerable. Even if there is but little gold, it may be of great advantage to separate it. The substances which, when distilled, have the natural Virtue of producing a Liquid that will dissolve silver, are Copperas, Alum, Saltpetre and Armenian Bole, Orpiment and Cinnabar. Various mixtures are made up to obtain the result, but those most commonly used are equal parts of Alum and Saltpetre, or two parts of Alum and one part of Saltpetre. Copperas and Saltpetre can also be used in the same proportions. When I have no glass vessels at hand for distillation, I usually add five or six ounces of drinking water to the mixture of one pound each of Saltpetre and Copperas, in order to provide for the initial absorption of the clay vessels. First prepare the aforesaid materials in the following manner: Charge the copperas into a vitrified clay pot, and heat until it melts; stir well with a thick wire; then remove from the fire, cool, and pulverize well. The saltpetre is also heated over the fire, cooled and pulverized. The alum is 256
FlF.'DACIĂ“N JCANELO TURRIANO
prepared in the same way as the copperas, though sorne calcine it on an Iron sheet and then pulverize it. The glass vessel in which these materials are charged is called, on account of the likeness, the chamber-pot. First coat the lower half, at least, of the vessel, with mud in this way: Make up a liquid mud, like porridge, from a good class of kneaded clay; wet woolen strips, or, if they are lacking, soak wool or clipped hair in the liquid mud, and apply as a thin coat to the retort. Let dry and repeat until a coating of one finger-thickness results. If the distilling furnace needs to accommodate but one retort, make it from adobes, about eleven inches square inside. Provide an ash door at the front, six to eight fingerthicknesses in width and proportionally high. At a point about eleven inches from the ground, provide a grate made from small bars or a perforated plate, in order to support the coals and at the same time to allow passage to the ashes. Leave another 'door above the grate for charging wood and charcoal. Build the side walls another eleven inches higher. Cover the furnace with a sheet of Iron supported by two iron bars extending from wall to wall. Let this sheet have four holes in the comer for maintaining the draft, and a large hole in the centre capable of receiving a clay vessel into which the glass retort is fitted. The clay vessel must be large enough to allow the glass retort to be set into it and packed around with sand or ashes. Having ground and mixed (in the proportions indicated) the powders from which the acid is to be distilled, charge the retort one-third or, at the most, one-half full. Put on the hood, and lute the joint well with sorne strips of linen soaked in white-of-egg or flour paste, in order to prevent leakage. The nose of the hood is fitted into what is called the receiver, that is, a large flask, in which the distilled liquid is collected. This is also luted to prevent leakage. Light the furnace and heat slowly at the beginning until distilling commences; when the glass shows the colour (gas), increase the heat. Do this with such care, however, that FID.DACIĂ“N JUANELO TURRIANO
ARTE DE LOS METALES
at least five -minutes by tlie dock, or five bell sti:okes, and not more than ten, elapse between the falling drops. If the drops fall more rapidly there -is danger of breaking the retort; if they fall too slowly the work is prolonged more than is convenient. Remedy the first condition by removing sorne of the coals with the tongs, and the second by augmenting the fire by adding small sticks of dry wood and regulating the draft. It will be well to cover the receiver with sorne cloth wetted with cold water, in order to condense the fumes with which it is filled. When the upper part of the retort shows white, it is a sign that the materials have completed their yield of fume. Hold back the fire until drops cease entirely; remove the coals from the furnace and allow the vessels to cool.
FU>-IDACIﾃ的\ JCANELO TURRIANO
CHAPT ER EIGHT CONTINUES WITH THE SUBJECT OF THE LAST CHAPTER; AND ADDS SOME WARNINGS IN REGARD THERETO
In place of vessels or chambe r-pots (retorts) of glass for distilling the material s for Nitric Acid, even well-ma de vitrified clay vessels of the same shape may be used, with good results; it will be sufficient that the alembic and receiver are of glass. A number of these retorts may be placed side by side in long box-like furnaces built of adobes and bricks of the same type as those used for calcining slimes. They are all heated from the same grate. In this way an abundan ce of nitric acid can be obtained for the parting of Gold and Silver. It is of much importa nce to know whether the Silver carries Gold, especially to those working in new and outlying mining districts . Even if glass hoods and receivers are lacking, it is well to know how, on occasion, to obtain sorne nitric acid, even if but little, in arder to determi ne the Silver in the assays. The material s exist everywh ere. It will suffice that the receiver be of vitrified pottery, such as a small jar, or vial, even if the vessel in which the materia l is distilled is not vitrified. Place tightly together the mouths of the vessels used as retort and receiver ; lute and cover well; even if much liquid is absorbed , enough will be recovered for an assay which will give the desired informa tion. Thus I did when I lived in Los Lipes at first, when that Provinc e had but few Spanish inhabita nts and there was a lack of all sorts of facilities. Leave a hale, the size of a large iron Needle, between the retort and receiver ; clase with a small wooden Peg which can be removed if the fumes from the distilling compou nd 259
FUNDACIĂ“N JUANELO TURRIANO
ARTE DE LOS METALES
become too powerful and dense. Thus the air imprisone d in the receiver will be cooled, the gases will condense more quickly, and there will be less risk of breaking the vessels. When the Nitric Acid has been removed from the receiver, pour a little in a flask and on half a drachm of silver. When the silver is dissolved add a small amount of water; add more water, and in a short time the liquid, which at first appeared turbid, will become clear, and white sediment will fall to the bottom. Separate this sediment and save in another tightly stoppered flask or vial. When the vessels are cold, remove from the retort the calcined and exhausted residue remaining after distillatio n; if very hard, it is best to add water, to avoid the risk of breaking the retort, and heat moderate ly in order to dissolve and easily remove the material. I invented a kind of vessel for distilling Nitric Acid, which is so well adapted for this purpose that I have continued to use it, and have passed it on to my friends. The best vessels for these distillatio ns are long-necked glass retorts, because of the short travel for the fumes coming off from the materials ; they, however, are inconven ient on account of the difficulty of filling and emptying through the long and narrow neck. Make an imitation (of the foregoing) of good clay, and on top, before the clay dries, describe with a compass, and cut out, ĂĄ piece the size of a crown, large enough to admit the hand easily; place four protrudin g buttons or knobs equally distant around the circumference of the opening. Bake and glaze both the retort and the piece cut out, which is to serve as a lid. Charge the materials through this handhole , put on the lid, adjust and lute so that the vapours cannot escape, fasten the cover with a wire which passes diagonall y around the buttons, and connect to the neck. When the distillatio n is finished the materials can be removed with the greatest facility through the aforesaid openmg. FUNDACIĂ“N Jt.:ANELO TURRIANO
A-Furnace. B-Fire-daar. · C-Daar- to ash-pit. D-Large hale in the sheet cavering the furnace. E-Small draft hales. F-Grate bars. G-Chamber-pat (retart) af glass or vitrified pattery. H-Haad af the still. 1-Langnecked vitrified pattery retart. K-Hale the size af a crawn, in the tap af the retart. L-Caver far this hale.
FUNDACIÓN JCANELO TURRIANO
CHAPTER NINE HOW TO ASSAY SILVER TO DETERMINE IF IT CONTAINS GOLD
Although one can obtain a fair idea of the proportions of the two Metals by using the test needles with care, the method is not so exact as might be desired; nor is it well to trust to the sight alone in such an important matter. If the silver carries half a carat or half a grain of gold, the needles will scarcely show the difference between it and a sample which carries no gold; this means, in twenty-four ordinary bars of three hundred and twenty ounces each, a difference of ten pounds (avoirdupois) of pure Gold, whose value is known to us all. Precisely for this reason, the assay by Nitric Acid is necessary, in order to determine if there is an admixture of Gold, and in what quantity, in order to recover if sufficient. When the nitric acid is made the rest is easy. Proceed in the following manner: Cupe! the silver with a little lead in order to remove any copper or foreign metal it may contain, and so that nothing but gold will remain with it. If available, have ready a glass or a small china cup, though the best thing of all is a twenty-four carat gold cup. This I have used for many years; it lasts forever, and is damaged neither by ordinary nitric acid nor fire. lt may be placed without danger directly on the coals, while the glass can only be put in the ashes. Beat the silver into thin sheets; cut them into pieces the size of a finger-nail and double them into cornets. Clean them well and weigh out the quantity to be assayed, taking the largest of the set of small assay weights. Place the weighed piece in the aforesaid cup and pour on Nitric Acid to cover. Put on the 262
Flr.\DACIÓN JCANELO TURRIANO
fire and boil. gently. If a glass cup is used, it may be necessary to add more boiling acid; with a gold cup this precaution is not necessary. So long as there is Silver for the acid to attack, bubbles of smoke wíll come off; when they cease, take the cup from the heat. If there is Gold it will be seen in the bottom as a black powder, or a residue like powdered brick. Pour the liquid into another cup; the Silver accompanies it. Wash the Gold with three or four changes of fresh hot water, and save, as it all carries sorne Silver; repeat this until the wash water is no longer cloudy. Drain at once, and heat the Gold in the silver pan, and weigh when cold. The proportion of Gold in the silver can be determined by the table in Book Three, Chapter Eight; the value of the gold in each hundred pounds of silver, based on eighteen Reales to the Castellano of twenty-four carats, can also be determined by the same table. When the silver contains much gold, or when the gold contains sorne silver, it is assayed and parted in the following manner: First of all remo ve the copper from the bullion by refining with lead, in the cupelling furnace. Determine the fineness with test needles of gold and silver. If the proportion of gold is high, it will defend the silver against the desired action of nitric acid, and it will then be necessary to reduce the proportions to two of silver and one of gold; this really means that gold of a higher fineness is reduced to eight carats by adding the necessary silver. Experiments have proven this to be the best mixture tci prevent the gold from being excessively divided, and yet, at the same time, allow all the silver to be dissolved. · Let the silver which is to be added be assayed, in order to have the satisfaction of knowing that it carries .rÍo gold whatsoever; if it does, the assay will not be exact~ . . :For · --th.é rest, proceed as befo re indicated. If the gold fineness is high and it has to be reduced to eight carats by alloying with silver, the quantity which must be added to each Peso weight of bullion of a determined fineness can be determined from the accompanying table, which FUNDACIÓN JCANELO TURRIANO
ARTE DE LOS METALES
shows the Pesos (2% drachms) and Tomines (i drachm) opposite the fineness in carats. For example, if it is desired
Carats 24 23 22 21 20 19 18 17 16
Pesos drachms) 2 1 1 1 1 1 1 1 1
(t drachm) o 7
15 14 13 12
Pesos Tomines drachms) (i drachm)
o o o o o o o o
5 4 3 2 I
to reduce twenty carat gold to eight carats, the table shows that one Peso four Tomines of gold-free silver must be added to each Peso of the aforesaid fineness. When melted together they will amount to two P esos anda half of eight carat bullion. However, it often happens that gold of a high fineness must be alloyed with silver which contains sorne gold. In that case the calculation must be made as in the following example: If it is desired to reduce twenty carat gold to eight carat, using silver which contains two carats of gold, put them down in this order: 20 . . . . 8 . . .. 2. The difference between 20 and 8 is 12; place it abo ve the 8. The difference between 2 and 8 is 6; place it above the 2. The tabulation will then be: 12 .••. 6 20 .•••
8 .... 2
I divide the first remainder (12) by the second (6) and obtain 2; this is the number of Pesos of silver, two carats fine in gold, which must be added to each Peso of twentycarat bullion to reduce to eight carats. If, on the contrary, it is desired to raise two-carat gold · to eight, with FU1\DACIÓN JCANELO TURRIANO
high-grade gold of twenty carats, put the numbers down in this arder: 6 .... 12 2 ....
8 .. . . 20
Divide the first difference (6) by the second (12); the result is !; therefore, to each Peso weight of two-carat bullion, half a Peso of twenty-carat bullion must be added to bring it up to eight carats. Other calculations are made in the same way.
FUXDACIĂ“N JCANELO TURRIANO
CHAPTER TEN HOW GOLD IS PARTED FROM SILVER
Gold is parted from silver in the same way as in Assaying, described in the last Chapter; the only difference is that for large-scale work the vessels and other equipment must be proportionate ly larger. The work may be carried out in glass vessels, though he who obtains vessels of fine gold will save much. I have been obliged to use gold vessels on account of the scarcity and cost of glass, and the risks attendant on its use, dueto the frequent Breakage in this rigorous climate, even when the greatest care is exercised. Take gold and silver Bullion, alloyed in the proportions indicated, and granulate finely; the less rounded the granules the better for the work. Or, the bullion may be beaten into thin sheets, cut into small pieces, annealed and made into cornets. Pour nitric acid over the cornets so that they are covered to a depth of two or three finger-thicknesses. Boil until all the silver is dissolved; this condition will be recognized by the sign already described under assaying. If necessary, add more acid. Lastly, transfer the liquid, in which the silver is dissolved, to a copper Kettle, adding an equal quantity of water. The silver will deposit at once on the copper vessel. If preferred, the diluted liquid may be transferred to vitrified Clay Vessels, containing sorne bars of copper on which the silver will deposit. The silver is all deposited when a cloth tape inserted in the liquid does not blacken or change colour. Or, a salt brine can be added to the liquid carrying the dissolved silver, and it will at once settle to the bottom. By any one of these methods the silver may be recovered. Dry the residue well befare melting; if it has much adhering 266
_ FU)JDACION JL:ANELO TURRIANO
moisture the surface will be blackened, and on melting it will burn and there will be sorne loss of silver. By all of these methods the nitric acid is lost. He who cares to recover it, however, may do so by distilling the silver-carrying liquid, whereupon nitric acid with all its former strength will be recovered for a second use. The Silver will remain in the retort and may be melted, with the precautions already cited. The Gold which remains in the bottom of the parting cup is washed three or four times· with pure water, or until the wash water is no longer cloudy. It is then dried, removed and melted with a little borax; or Corrosive Sublimate may be added to soften it, as is done by Jewellers (Silversmiths) . The wash waters should be saved, as they also carry silver. They may be distilled, and the first portion which comes off will serve for washing gold; that which distils off after the coloured fumes begin to appear will be strong, and may again be used for parting.
FUNDACIÓN JUANELO TURRIANO
CONCERNING OTHER METHODS FOR PARTING GOLD AND SILVER
Although the most convenient and exact method of parting gold from silver is by means of Nitric Acid, not every one will apply himself to its distillation; nor are there always the necessary Elements for the large-scale work, as described in the last Chapter. However, in any case it is necessary to use nitric acid in assaying Silver to determine if it contains Gold, as has already been stated. There have been invented various other methods of refining Gold, all founded on the fact that its Purity and Lustre are altered with difficulty, while the other metals, on the contrary, are easily altered or contaminated. E ven the purest Silver is so dulled and contaminated by Sulphur, and is thereby reduced to a substance so Black and Brittle that only a person very expert in these matters can tell it from a slag. Antimony does the same, because, as stated in the description thereof, it abounds as a compound of sulphur. Using these two materials, Silver and Gold are parted _ in the following manner: . Granulate the Silver bullion, and to each twelve ounces add two ounces and a quarter of well-ground unsublimed Sulphur. Mix well and charge into a new clay pot, well covered and luted. Heat gently, so that the Sulphur will melt and mix with the Silver, but will not burn. Remove the black Silver (Sulphide) from the pot; have ready three ounces and a half of granulated Copper for each twelve ounces of the original Silver. Charge the black Silver with half of this granulated Copper into a crucible; cover and fire until melted. When melted, add a spoonful of granu-
FlF.\DACIĂ“N JCANELO TURRIANO
lated Copper and a spoonful of a mixture made with equal parts of Lith'arge, granulat ed Lead, calcined Salt and Borax; cover the crucible, and when the charge is melted add, in the order mention ed, the balance of the granulat ed Copper and composition. Through this operatio n the Gold will go to the bottom of the crucible, while the Silver will come to the top and be mixed with the copper-lead matte, mentioned before. T o ascertai n the depth of gold in the bottom of the crucible, insert a clay-covered iron wire and remove it at once. That part which is white indicates the depth of gold; the blackened part indicates the depth of matte and slag. When the charge is well cooked, empty it into a mould; the gold can then be easily separate d from the matte. Before removing the crucible from the fire, take out a little of the matte and cupel with lead; dissolve the Silver Button with nitric acid to determin e whether the parting has arrived at the desired degree; if not, continue heating the crucible. The Silver and Copper may be parted and recovered in the manner already described. Sulphur also will separate Gold and Silver, though the procedu re is somewh at complicated. Make a strong brine which will fl.oat an Egg, as described for the manufac ture of Sal Artificiosa [This was apparen tly a stock flux.- Translators]. BoĂl powdered sulphur in this brine until it will melt over a naked fl.ame, like wax, but will not ignite. When the sulphur thus prepared is mixed with melted gold and silver bullion, it will separate them.
FUNDACIĂ“N JUANELO TURRIANO
CHAPTER TWELVE HOW GOLD AND SILVER MAY BE PARTED BY USING ANTIMONY AND CERTAIN OTHER COMPOUNDS
1 1.1 1: â€˘
Melt eight ounces of Antimony and half an ounce of Copper in a clay crucible. Have ready three parts of this mixture to each part of bullion to be parted. Add a little of the Antimony mixture to the melted bullion; when melted in, add the rest little by little, waiting for each lot to melt well before adding more. Cover the crucible and allow to heat for as much time as one would spend in walking thirtyfive or forty paces. Have at hand a conical iron crucible (mould) greased and heated, and supported on a wooden foundation, in order to receive the melt. Tap the mould so that the gold will settle to the bottom. When cold, remove the Gold Button and melt again with the antimony mixture until the desired fineness has been attained; however, it will not be necessary to use so much Antimony as the first time. Finally, refine the Gold Button on a cupe!. To the antimonial residue add an equal weight of Argols and half as much Borax. Melt the mixture on a piece of tile or in a clay crucible two or three times; any gold which may have remained will settle to the bottom as a Button which can be melted and refined like the first lot. After this, add Lead to the antimonial residue and cupel the mass to recover whatever Silver it contains. If the antimonial mass is not re-melted with Argols and Borax, Silver will be lost in the cupelling. Other compositions for parting gold and silver are made from Sulphur, Antimony, etc. The sulphur used is prepared by grinding well and boiling with strong Vinegar for six hours; it is then removed and washed with hot water. 270
FUNDACIĂ“N JCANELO TURRIANO
The first compound of this kind is made of one pound of the aforesaid Sulphur and two pounds of very well purified Salt. Another mixture is made of twelve ounces of Sulphur, six of Sal Artificiosa three of Red Ochre, and one of Minium. Another consists of half an ounce of Copperas, well dried over the fire, two ounces of Sal Artificiosa, four of Antimony, six of Sulphur, one quarter of an ounce of glass, one quarter of an ounce of Saltpetre, and one eighth of an ounce of Red Ochre. The fourth mixture consists of twelve ounces each of Sal Artificiosa, prepared Sulphur, and Shavings, and six of Borax. Still another consists of equal parts of the aforesaid Sulphur, Red Ochre, Saltpetre and Copper Oxide. T o twelve ounces of well-melted gold-bearing silver, add two o unces of any one of the aforesaid powders; stir very well and pour into another well-heated crucible which has been greased with tallow. Shake this crucible so that the gold will settle to the bottom; for the rest, proceed according to directions already given. Gold may be separated from pieces of gilded Silver, without detriment to them, in the following manner: Grind to a powder half a part of Sulphur and one part ·of Sal Ammoniac; grease the piece, dust with the aforesaid powder and use the tongs to place on. well-lighted coals. When well heated, shake the piece over a tub of water, into which the Gold will fall, and from whence it can be recovered. The same effect can be obtained by immersing the gilded piece in hot Quicksilver until well amalgamat ed. Remove and plunge into cold water, and the mixed Gold and Quicksilver will drop off: Repeat this as many times as necessary until there is no sign of Gold adhering to the piece. Squeeze and retort the amalgam in the ordinary way used for silver.
FUNDACIÓN JL:ANELO TURRIANO
CHAPTER THIRTEEN CONCERNING THE PARTING OF GOLD FROM SILVER, OR ANY OTHER MIXTURE, BY WHAT IS CALLED CEMENTATION
Damages of great magnitude have been caused by that action which is called Cementation. Ignorance of this marvellous action on metals has caused the loss of great sums of Silver, because the Precautions given in Chapters Eight and Nine, of Book Two, were not applied. In the Cementa• tion Process of parting, there is a burning of metals or alloys, against which Gold alone, by reason of its unequalled Nobility, is proof. Various materials enter into these Cementation compounds, the proportions cited by different Authors depending on their experience in refining gold. However, all the Elements of the compounds are mineral, and of the kinds which ordinarily accompany ores that are roasted before amalgamation ; this is a proof of the Losses and Inconvenience s before mentioned, because when the Silver is calcined it is easily dissolved; being dissolved, it is not recovered, and therefore the Metallurgists say that it was volatilized in the furnace and that the charge was overdone. In Ulphstadio's treatise on Alchemy, in the writings of Agrícola, and elsewhere, are to be found Formulae of various cementation compounds. I do not consider it necessary to give them, because the ordinary mixture is easily made from ground brick and common salt, or rock salt, in the following way: T ake nine o unces of sifted brick powder and mix with three o unces of salt, using these same proportions on a greater or lesser scale, according to the quantity of Gold to be parted. Beat the Gold into thin sheets, like Escutcheons, or 272
FUNDACIÓN .fl:ANELO TURRIANO
even thinner. Moisten the aforesaid mixture with strong vinegar in which has been dissolved half an ounce of Sal Ammoniac. Put a bed of this powder on the bottom of a new clay pot; on the powder place a layer of the gold sheets in such a way that they are not touching. Cover the gold with a layer of powder, and continue alternating thus until the pot is full or there are no more gold sheets. Frequently the gold sheets are wetted in a vinegar solution of Sal Ammoniac before charging into the pot. Cover and lute the pot well. Place it in a round or square furnace duly provided with grate bars and ash-pit. Heat evenly until redhot in all parts, like the retorts in which amalgam is distilled. Continue heating evenly so long as necessary, depending on the fineness of the bullion charge. Among jewellers it is accepted that bullion will increase one carat in fineness with each twelve hours' firing, but this is not infallible, nor is so much time always required. When the charge is thought to be finished, remove the pot and· cool. Try the bullion with the test needles, and, if not totally fine, or of the desired fineness, charge the plates again with fresh powder and repeat the heating. The Silver contained in the bullion will be taken up by the powder, and may be recovered therefrom by the method given for the amalgamation of ores.
FUNDACIÓN Jt.:ANELO TURRIANO
CHAPTER FOURTEEN THE ACIDS WHICH DISSOLVE GOLD
The elements which, when resolved into liquids by distillation, have the power of dissolving Gold are Vitriol, Saltpetre, Sal Ammoniac, Antimony and Corrosive Sublimate; various compounds may be made from them. The first compound is made with two pounds of Vitriol and an equal quantity of Sal Ammoniac; distil in the same way as when making nitric acid, or take one pound of nitric acid in which silver has been dissolved and add three ounces of sal ammoniac; when dissolved, distil in a glass retort, and the resulting distillate will dissolve Gold; or use one pound of saltpetre and an equal amount of antimony, or equal parts of saltpetre, salt of urine or sal ammoniac. Raymond dissolves Gold. in the Fifth Essence of Wine, highly rectified (with the help of a salt prepared from the same essence), in arder to make his Potable Gold and the Stone so celebrated among Philosophers. However, the easiest method for dissolving Gold, and the one I have found most suitable, is to add one ounce of well-ground and easily dissolved household salt to each four or five ounces of nitric acid. The liquid totally loses its former force for dissolving Silver and acquires a violent activity against Gold (which it at first did not attack), converting it toa ruby liquid. This inspires the merited admiration of all who give due consideration to the reasons for these contrary effects. F or many years, in these Parts, I ha ve used cups of the finest Gold for parting Gold from Silver, as befare mentioned, on account of the lack of glass and the risk in using it. On one occasion, when I was making an assay, the parting acid lacked strength; while it was still boiling I added a little 274
FUCJDACIĂ“N JL:ANELO TURRIANO
salt, which I happened to have at hand, thinking it might · give greater penetration and be of help. No more Silver whatsoever was dissolved, though the liquid started to become yellow. At this novelty I paused, when I saw that the Gold was being dissolved. I have used this procedure many times since, in glass cups; it is both curious and easy. If there is but little silver in the bullion, it will settle to the bottom of the cup as a fine powder; if much, it will remain as spongy and brittle sheets or tubes. Pour off the liquid carrying the gold; wash the silver three or four times with hot water, until it is no longer yellow; save the wash waters, as they all contain gold. Afterward, melt the silver when well dried. D:stil the gold solution if it is desired to recover the acid; if not, evaporate to dryness over a slow fire; the residue will be gold and salt. Melt in a crucible, using a strong heat, until the gold residue melts, or at least until the salt can be separated from the gol d. One of m y personal experiences (and non e the less esteemed on account of the greater discoveries it may lead to) is the separation of the Gold from the Salt. It is done in the following manner: Grind very finely, on a stone, the welldried yellowish gold chloride and salt residue; charge the powder in a glass vesse1 and cover with water-free, well-rectified alcohol to the depth of two finger-thicknesses. In a ve~y short time the Fifth Essence will dissolve all the gold chloride and take on its yellow colour, though it will not dissolve the least quantity of the white salt. Pour off the yellow liquid and wash the salt once or twice with more alcohol until it remains white as snow, and the liquid is no longer discoloured. This Fifth Essence solution of Gold chloride will be sharp to the taste, on account of the copperas used in making the acid. It is a subject appropriate for Chemists, but one of which I am careful not to write. Even on previous occasions I have passed over this in Silence, in order not to embark on the pursuit and study of an Art which, though feasible and exact, has caused, and still causes, the greatest harm to FUNDACIÓN JUANELO TURRIANO
ARTE DE LOS METALES
those who ordinarily exercise it without reason. Most rare in this World is it to find Persons who have obtained sorne advantage from their knowledge of the Art.
FUNDACIĂ“N JCANELO TURRIANO
INDEX A Abitanes, gold in, 66 Accidents occurring in amalgamation, 130 Acids which dissolve gold, 274-276 Adobes, furnaces of, 187 Agate of King Pyrrhus, 40 Agricola, Georg, 3, 57, 63, 104, 165, 197, 207, 212, 222, 237, 272 Agua caliente, crystalline stones of, 35 Agua fuerte (nitric acid), 14, 1n Albayalde (white lead), 27 Albertus Magnus, 18, 40 gold the only perfect metal, 49 margarita, 26 on constituents of stones, 28 on transmutation, so Alchemists find source of comets, lightning, etc., in vitriol, 45 theory of asto formation of metals, 44 Alcohol (antimony), 98 Alloys and artificial metallic compounds, 84-87 brass, how made, 84 bronze production, 84 cadmium, 85 cardenillo (verdigris), 86 cinabrio (cinnabar), 84 copper fiour, 85 copper scales, 85 enamel, 85 glass, 86 greta, 86 itch cures, 85 mercury, 85 metal mixtures for mirrors, 84 pompholyx (zinc oxide), 85 purpurina, 86 sandix, 86 slag, 85 277
Alloys, solimĂĄn (corrosive sublimate), 8s spodium, 85 verdigris, 86 vermicular, 86 yellow ochre, 86 Almadaneta (hammer rock), 30 Almojatre (sal ammoniac), 18, 19 Alum of Escayola, 12 argols, 12 catino, 12 seysile or feather alum, 12 Alurns, n Amalgam, best method of retorting, 145-147 losses in retorting, 143 losses of, 142 silver yield one-fifth of amalgam, 142 squeezing and retorting, 142-144 surer methods of retorting, 145-147 Amalgamating gold and silver ores, 93-147 Amalgamation, boiling, clean-up on cold amalgamated charges, 18o, 181 correct method of recovering values from ores by, 165, 166 enormous losses of quicksilver, 94 excessive fiouring, 133 iron cauldrons to recover quicksilver, 18o iron to reunite fioured quicksilver, 133 magistrales, composition of, 131 mishaps of, and their remedies, 13o132 nitric acid as aid in recovering quicksilver, 18o, 181 precautions to prevent loss, 94 rich ores of gold and silver, 182-184 treating ores of silver by, 93, 94 tintin (mortar and pestle) treatment of rich ores, 183 Fln\TIACIĂ“N Jl:ANELO TURRIANO
Amalgamator, duties of before mixing Base metals, iron refining, 250 lead and tin, faulty refining, 249 charge, II7 refining, 249-251 warnings to in roasting ores, 120, 121 Amoladera (grindstone-sandstone), 31 Bautista, Leon, 40 Amontonadas (heaps, irregular ore Béguin, Jean, on oil of salt, 17 Berenguela de Pacajes, District of, 38 deposits),· 61 fire-assay of ore from abandoned Anco (irnpure native silver), 176 mine, 96 Ancoraymes-iron workings of Incas lethal odour from mine at, 5, 6 near, 76 Antimony (estibium, alcohol, maza- Betunes (pitches), 2o-22 Bismuth, 55 cote), 24 Blue caparrosa (copper sulphate), 108 and sulphur, 23-25 Bracesco on the source of metals, 45 how found, 25 Maricio frnds medicinal use for anti- Brass, how made, 84 Bronze production, 84 mony, 24 Buenos Aires, 34 to part gold and silver, 270, 271 Antipathies and sympathies existing Bullion, refining gold and silver, 244, 245 between ores, 151, 152 e between metals, 152 30 (barite), Cachi fuerte (nitric acid), 152 Cadmium, 85 Arica, xo , Calichal (white earth, kaolin) as bearer Aristotle on earth colours, x, 2 of gold, 59 on origin of metals, 41 Calisthenes, gold only perfect metal, 49 " Artificial Sal t," 2n on transmutation, so "Artificiosa," 254 Callapa, 35 Asphalt, behaviour of in flame, 21 wide copper veins near, 73 source of in Dead Sea, 20 _ (camphor tree), 20 Capar Assay, table for calculating, 204 alchemists' (copperas), Caparrosa Assaying ores by fue, 213-215 13 of, theory silver to determine presence of gold, evil odour of, 13 262-265 known also as rnisi, sori, calchitis, and Assays, small-scale tests on other ores, : melanteria, 14 ~ 219-221 oil of vitriol from, 14 Atacama, Province of, 13, 34, 66 taste of, 13 copper veins at, 73 transmuting powers of, 14, xo8, no curious stone altars, 3 7 x6 Caquingora, minerals and precious stones, 37 rich copper workings near, 73 pearls in, 36 Caraboya, gold in, 65 turquoises of, 35 Carabuco, tin mines of the lndians, 79 Augsburg, salts in mine at, 27 Avicenna, on constituents of stones, 28 ¡ Carbonilla (charcoal mixture), 187 1 Cardano, 9, 40 on steel-water, 153 sees black silver, 53 Cardenillo (verdigris), 86 B 1 Cardona on earth colours, 2 de Barondelet, D. Paulo, reviews anq Castellano (shaft) furnaces, 194 Cauldrons used in treatment of ores, approves Barba's book, v Base metals, copper refining, 249
xss-157 FlliDACIÓN JCANELO TURRIANO
Cauldrons, black silver ores not suit- Cleaning up the charge, r68 able to this method, I77 determining when charge is ready for, construction of, rss-IS7 I35, I3Ó copper only to be used in amalgafactors governing time of, I35 mation, ISS troubles confronting, I35, I36 cost of yareta as fue!, I74 Cochizo (pyrargyrite), 98 damages to, and how to remedy, I7o Cocos (coconuts), amethyst-bearing, disadvantages of, I69 explosive qualities of, 34, 35 drawbacks to this method and the Colcha, 12, r78 remedies, I7Ó-I77 Cold amalgamated charges, making fire-wood, consumption of in this boiling amalgamation clean-up method, I73-I75 of, I8o, I8I how to erect, IÓo-I62 Collecter with which silver ores are in large scale work, I7r, I72 smelted, 209 iron, for copper ores, I78 . Colours of earth, I, 2 size of, ISS of all minerals in general, 88, 89 Cementation method of separating of hills as indicative of presence of gold and silver, 272, 27J minerals, 59 Cendrada, 247, 248 recognition of ores by smoke, rr6 Cerro de Potosí, 8 Colquiri, 203 Chacapa, 22J, 247 tin mines of, 79 Cha1Iatiri mines, 47, 82 "Compendium of Transmutation," Charcas, District of, gold in, 65 Raymond's, 33 mercury deposits in, 82 Conchucos, Province of, 27 Charcoal as fue!, I97-I99 Confrustaño, 249 Chayanta, 12, 59 Constantinople, curious marble slab in, gold in, 66 40 tin in, 79 Cooking ores of gold, silver and copper Chichas, Province of, I45 (pan amalgamation), I49-I84 copper deposits, 7J amalgam from copper ores by, I78, lead in mines of, 78 I79 Chilleo, gold in, 66 discovery of this method, I49 Chocaya, JO improvement in method, ISO mines of, ÓJ iron cauldrons for copper ores, I78 Choquepiña, native copper at, 74 mercury losses obviated by, r66 Chrysocolla (atincar, borax), I8 monopoly granted to author, ISO Chumpi (magnetite), JO, 76 silver-bearing copper ores yield full value, I78 Chuquisaca, 57 treating ores by, I63, r.64 gold in, 66 treatment of ores of gold and silver Chuquichuqui, gold in, 66 by, I49-I84 Cibairo, I78 Copaquiras, I3 Cimiento (cementation powder), rri Copper and its ores, 72-74 Cinabrio (cinná.bar), 84 Atacama, massive outcrops at, 7J Ciques (rhyolites?), JI Callapa, wide viens of, near, 73 Classification of substances formed in Caquingora, workings at, 73 the earth, I, 2 cause of colour in, 53 of stones, JO, JI Chichas, mines of, 73
FID:DAC IÓN JCANELO TURRIANO
Earth and her tastes, 7 Earths, 8-u 74 almagre (red ochre), 8 colour of, 72 ampelites, 9 Curaguara de Pacajes, Indian workas medicines, 8 ings near, 73 aster, 9 durability of, 72 azabache (jet), 9 Esmoraca, mines of, 73 bolarmenico (Armenian bale), 8 formation of, 72 bolarmeno oriental, 8 Lipes, mines at, 73 britannico, ro mine at Oslloque yielding, 72 chia, 9 Oroncota, mines of, 73 cimolia, 9 parting from gold, 254, 255 definition of, n parting from silver, 252, 253 guano, ro Sabalcha, mines of massive native, 73 lemnia, 8 Tarabuco, mines of, 73 names and uses of, 8-ro Tarua, mines of, 73 of Erithria, 8 the origin of silver mines, 73 of Samas, 9 Turco, deposits in, 73 phigite, 9 Yulloma, fine quality of viens at, 73 selinucia, 9 Yura output, 73 the eleven compounds, u Copper flour, 85 Eliana on converting mercury into Copper scales, 85 lead, Sr Copper sulphate a cause of loss of Elphstadio's treatise on Philosophy, 153 quicksilver, 139 Elpidiano, Andres Baccio, Thermis of, in amalgamation, 130
Copper, Choquepiña, native deposits at,
Copperas, 13, 14, 121 enemy of quicksilver, 125 Cordones, 242 Coroyco, gold in, 65 Curaguara de Pacajes, Indian copper workings, 73 Cupelling bottoms for refining gold and silver, 241-243
De Galileis, Galileo's, 56 De Re Metallica, Encelius, iv Determination of ore value by fue assay, 167, 168 Dioscorides, u on margarita, 26 on waters of the metals, 153 Dioscorides of Matiolo, 21 Ductility of metals, 53
E Earth and her colours, r, and her smells, s-<>
Empedocles, 151 Enarnel, 85 Encelius, De Re Metallica, iv Entremoz, Portugal, mud odours of, 3 Epatica sulfuris·of Theophrastus, 23 Erithria, earths of, 8, 9 Esmoraca, gold in, 66 native copper at, 73 Estibium (antimony), 24 Experiments to prove damage from roasting ore, uo-n2
F Ferrariense, Count Hercules, 21 Ficiño, Marcillo, on potable gold, 154 Fire-assay a necessity, 96 necessity for prospectors knowing, 213 warnings as to, 216-218 Fire-wood, consumption of in cauldron method, 173 Fixed stars, as sources of precious stones, 55 FUNDACIÓN JUANELO TURRIANO
INDEX Floured quicksilver, 124, 125 causes of, 124 copperas enemy of quicksilver, 125 Fluxes, 209, 210 Furnaces, smelting, materials of, 187 braguetilla (pit furnace), 200 castellano (shaft), smelting in, 194, 229-235 charcoal as fuel, 194 earthen vessels as, 193 for finely ground ores, 188-191 for separating silver and copper, 200 lump ore, 192, 193 muflle construction of, r88-r90; 198, 199 . parting and refining, 2oo-202 pit, 194. 195 rectanguaar, forlumpores, 192 reverberatory, 188, 192, 194 round, 197 smelting with charcoal, 197, 198 tocochimbos or muflle, 194, 198 varieties of, r88-191 wind (guayras), 198 wood burning, 194-196 G Galen, 11 on waters of the metals, 153 Galena ores, reverberatory smelting of, 226-228 Galileo's De Galileis, 56 Garci-Mendoza, salt fields of, 15 Gemna (stone salt), r6 Genesis of stones, 28, 29 Glass, 86 Gold, Abitanes mines in, 66 acids which dissolve, 274-276 antimony to part silver and, 270, 271 as a rejuvenator, 64 assaying silver to determine presence of, 262-265 cause of variation of colour in, 53 cementation method of separating silver and, 272, 273 Chayanta, District of, 66 Chilleo, gold in, 66 Chuquichuqui, mines at, 66
Gold, Chuquisaca, mines at, 66 Colcha workings, 66 cupelling bottoms for refining, 241243 Esmoraca, gold in, 66 fineness of Carabaya ore, 65 incorruptibility of, 64 La Paz, mines of, 65 ni trie acid to part silver from, 256-258 Oruro, mines at, 66 Paccha, mines at, 66 parting from copper, 254, 255 parting from silver, warnings, 25926l, 266, 269 Presto, mines at, 66 qualities of, 64 refining, warnings in regard to, 246248 removing from gilded copper, 255 separating from gilded silver, 271 sulphur as agent in separating silver and, 269, 270, 271 table for reducing fineness of in as5aying, 264 usually found in red or dark yellow soil, 59 Green caparrosa (ferrous sulphate), ro8 Greta (litharge), 86 "Grinding-in," 128 Grinding ores, 104, ros Guaco de Santiago, 134 Guarina, mercury mines near, 83 H Henry of Saxony, 3 Heuchiente, Diodoro, 24 Hornos Castellanos (Spanish furnaces), 197 Huancavelica, 47 mercuiy mines at, 82 petrifying qualities of water of, 28 Hyacinth (tartar emetic), 24
1 llua (Elba), conversion of earth into iron at, 44 Individual metals, 64-66 "Intellectual Art," Raymond's, 123 Fll'JDACIĂ“N JUANELO TURRIANO
!ron, 75, 76 Ancoraymes, Inca workings near, 76 evils and advantages of, 75 method of smelting, 236, 237 not mined in the Province, 7s Oroncota valley deposit of, ¡6 properties of, 75 refractoriness of ores containing, IIS San Erigida, exposed vein of near, 76 Itch cures, 85
Los Lipes, copper mines of, 73 mines of San Cristobal de Achecolla, 1$
salt in, 15 Lump ores, furnaces for roasting, 192, 193 M Machacado, 182 Magara, conchitas of, 41 Magistrales, 131 Malacca, India, mud odour of, 3 J Mantos (blanket veins), 61 Jericho, 20 Maray (rocking stone) method of L crushing, 183 Margarita (pyrite), 26 Lagunillas, copper mines at, 73 colour and odour of, 26 Lamacradria, 30 damaging to ores, 26 Lampasceno, Straton on earth colours, 1 origin of, 26 La Paz, 73 varieties of, 26 gold mines of, 65 Marido cures ulcers with antimony, 24 transparent stone font at, 38 Marienburg, pleasing smell of mine at, 3 La Plata, 29, 129, 233 Larecaja, Province of, precious stones Matiolo, 21 Mazacote, 98 of, 35 Largo, Scribonio, on waters of the Medicinal virtues of mineral things, 8, 9, 90,91 metals, 153 Meissen Mountains, figured rocks of, 41 Las Chichas, 196, 203, 225, 226, 247 Mejillones, pearls in, 36 Lead, 77, 78 Mercury, 81-83, 85 Andacaba, in mines of, 78 Chalatiri, mines at, 82 a necessity in treating ores, 77 convertible into all metals, 81 humidity of, 77 Eliana on converting into lead, 81 in Chichas mines, 78 Guarina, mines near, 83 qualiti.es of, 77 Huancavelica deposits, 82 seldom found wii:hout silver, 77 loss of in silver extraction, 82 Sibicos, veins at, 78 method of avoiding loss of, 102 Lemina, 21 methods of obtaining, 238, 239 Lis (floured quicksilver), 124, 125 Moromoro, mines at, 83 Litharge, 86 qualities of, 81 Lizarán, Señor Don Juan, iv Raymond on conversion into gold Llama and cow dung as fuel, 192 and silver, 81 Llampos (fines), gold and silver occur· uses of, 82 as, 7 with sulphur a component of metals, pleasant smell indicative of presence of, 4 47 Metallurgist, professional equipment Llipita, 97 needed by, 95, 96 "Loading-up," 127 _ knowledge of fÍre-assay requisite, 96 Los Lipes,· province of, 12, 24, 34, 35, 96, 126, 142, 145, 150, 169, 178, Metals, alchemists' theory of formation of. 44 195, 203, 259 FU);DACIÓN JL'ANELO TURRIANO
JNDEX Metals, Bracesco on source of, 45 characteristics of, s2-s4 creation of, 43-45 · definition of, u ductility of, 53 genesis of, agencies effective in, 49-5 r genesis of, heat and cold as agencies, 49
genesis of, place of, s6 gold, cause of varing colour in, 53 humidity in, 52 lustre in, 52 mercmy and sulphur components of, 46-48
mercmy, origin of, 45 mixtures for mirrors, 84 number of, ss, 56 odour in, 53 origin of, 43 places originating, ss, s6 pyrite, 45 refining and parting, 241-276 resistance to flame of, 53 smell and taste of, 53 sulphUI, 45 transmutation of, 49 vitriol the basis of generation of, 44 Millo (alum), as reagent, 134 Mineral colours, 88, 89 Mirrors, mixtUies of metals for, 84 Mixing ihe charge, what must be done before, II7-II9 fire-assays, II 7 floUiing of quicksilver, u8 Molibdena, 247, 248 · Molle (a Bolivian tree), 242 Mongrovejo, Don Toribio Alfonso, 27 Monserrate, 26 Montagu, Edward, Earl of Sandwich, ili Moromoro, mercury deposits near, 83 Morro of Arica (Arica Bluff), precióus stones of, 35 Muertos (dead ores), 77 Mulatos, 97 . N N ames and uses of sorne earths, 8-ro Naphtha, 21 Natá, Panama, mud odoqrs of, 3 .
Negrillos (black sulphides), 73, 97, 121 treatmenf of, ro6 New Potosí, amethysts in mines of, 34 ruby .silver of, 47 sil ver mfues of, 69 Nitric acid, parting gold from silver with, 256-258 vessel for distilling, 260
o Odours, lethal, in mines at Berenguela de Pacajes, s, 6 o.ffensive, of most ores, 4 of metals, 53 Oieo petroleo (petroleum oil), medicinal virtues of, 21 Oques, 77 Ores, agua fuerte (nitric acid), ruaids in smelting, 2II alcohol (antimony), 98 amalgamation and smelting, 99, roo amalgamation of.rich ores of gold and silver, r82-184 assaying by tire,· 213-215 bad e.ffects resulting .from roasting, roS, 109
cimiento (cementation powder), ru cochizo (pyrargyrite), 98 ·comparison of chúnk and finely crushed roasting, II3 copaquiras, antipathy of to quicksilver, ror damage from roasting, -rro-rp tire assay, warnings as · to qúantity of ores, 2r6-2r8 galena, reverberatory smelting, 226228
grinding, 104, ros, 128 how to find veins of, 57, 58 how veins are s·qught, 59, 6o iron refractory in ores, ns llipita, 97 losses through neglect to sort, 99 lump, fUinaces for, 192, 193 · manner begotten, r~r materials to be mixed With, to roast them, II5, u6 mazacote, 98 FUNDACIÓN JUANELO TURRIANO
Ores, meUlod of avoiding mercury loss, 102
mulatos (black ores), 97 negrillos (black ores), treatment of, 106
pacos (oxide), 97, 99 plomo (native silver), 100 pol vorilla, 98 precautions in roasting, 120 precautions in working over charges, 128
preparing for smelting, 207, 2o8 prospecting for, method of, 6o pyrite, recognition of in, 103 Raymond on substances antipathetic to quicksilver, 101 recognition and removal of bad substances in, xox-1o3 recognition of and varieties of, 97, 98
recognition of ores by smoke colours, 116
reverberatory smelting on a large scale, 222, 223 roasting, xo6, 107, 12o-122 rosicler (proustite), 98 shovelling or sorting, 99, xoo silver, collector for in smelting, 209, 210
small-scale tests on base ores, 21922:x
smelting on a bath, 224, 225 soroches (galena), 98 sorting before smelting, 207 suco (chloride), 97 sulphur a destroyer of metal, II5 tacana (silver sulphide), 97, 98, 99, lOO
things begotten with, x, 2 three general divisions of, 97 time of roasting, 120 treating with lime, 127 trees, bushes and plants as indicative of presence of, 6o vitriols enemies of mercury, xox whether all the quicksilver and ore should be charged together, 126, 127
Ores, whether roasted in chunks or crushed finely, n3, 114 working over the charges, 128, 129 Oroncota valley, iron deposit in, 76 rich copper veins at, 73 Oronesta valley, figured rocks of, 41 Pucara (fortress), 41 Oropimento (orpiment), 26 a sign of gold, 27 Oruro, 8, 12, 58, 59, 62, 225, 245, 247, 249. 253
gold veins at, 66 white earth of, 143 Oslloque copper mine, 72 p
Pacajes, Province of, x6, 24, 35 Paccha, gold in, 66 Pacocaba, salt springs of, 28 Pacos (oxides, gossan), 97, u7, 120, x2x, I22
pleasing odour of, 3 Padilla, Diego, royal commissioner, iv, V
Pan amalgamation (cooking), ores best suited for treatment by, 158, 159 discovery of, 149 reagents, needed in, :xs8, 159 treatment of gold and silver by, I49-
x84 Paracelsus, 24 Pereyra, Province of Los Lipes, 59 Piedra iman (magnetic iron ore), 115 lipes (copper sulphate), 13 Pis-asphalt, 21 Pit furnaces, 195, 200 Pitch, sources of various kinds of, 20 varieties of, 20 Plato on origin of metals, 43 Pliny, I3I on orpiment, 27 Plomo (silver), 30 blanco (white lead), 79 falso (false amalgam film), 125 Polvorilla, 98 Pompholyx, Bs Porco, x:z, 235 FUNDACIĂ“N JUANELO TURRIANO
INDEX Porta, 24 Poton, 35 Potosi, iü, iv, 12, 16, 30, 58, 59, 64, 66, 73,78,92,134, 144,173,185,238
Precious stones, 32, 33 artificial, 33 fixed stars as sources, 55 flaws and their causes, 33 indications of in Bolivia, 34-36 qualities and origin of, 32 Presto, gold in, 66 Properties and virtues of mineral things, 90, 91 minerals as medicines, 90 Purpurina (tin purple), 86 Pyrite, 45 orpiment and dragon's blood, 26, 27 recognition of in ores, 103
Raymond, on conversion of mercury into noble metals, 81 on substances showing antipathy to mercury, 101 Rectangular furnaces for lump ores, 192 Refining and parting metals, 241-276 base metals, 249-251 gold and silver bullion, 244, 245 gold and silver, warnings in regard to, 246-248 Regulus, derivative of antimony, 24 Retorts, cast brass, 145 iron or copper, 145 Reverberatories, smelting of galena ores, 226-228 smelting on large scale, 222, 223 Rich ores, amalgamation of gold and silver, 182 Roasting ores, 106, 107 Rosicler (proustite), 98 Royal Commission of Potosí, recommends Barba's work, iv de Rupercisa, Juanes, u, 14
Quicksilver, nature of, 123 copper sulphate a cause of loss of, 139 iron cauldrons, use of to recover, 18o · loss by flouring, 133 loss of in washing charges, 137, 138 S losses in retorting, 143 Sabalcha, 178 losses, obviating, 18o copper mines of, 73 losses of thxough error, 137, 138 Sal ammoniac, 18, 19 methods of avoiding loss of, 140, 141 Sal artificiosa, 269 method of obtaining, 238, 239 Salt, 15-17 movement of stirrer a cause of loss, boiling lake of, at Tumaquifa, 16 139 difference between rock and sea, 15 purifying, 251 rock salt as a rejuvenator, 16 remedies for losses of, 139-141 virtues of an oil of, 17 salt a cause of loss of, 139 Salts, the, u slimes as a cause of loss, 139 definition of, u Quijo (quartz), 30 Samos, earth of, 9 San Erigida, iron deposit at, 76 R San Cristobal de Achecolla, mines of, Raris, on steel-water, 153 15, 58 Raymond, 11, 14, 126, 209 San Cristobal de Los Lipes, 63 copperas and gold have same origin, accidental discovery of mine at, 58 13 evil-smelling mine at, 4 dissolves gold in fifth essence of wine, mine at, abandoned because of foul 274 odour, 4 "Intellectual Art," 123 Sandaraca (dragon's blood), 26 on colour of precious stones, 32, 33 Sandix (red lead), 27, 86
FUl\'DACIÓN JCANELO TURRIANO
de Sandoval, D. Andres, royal commissioner, iv, v Seapi, Province of Los Lipes, 59 Shovelling or sorting of ores, 99 Sibicos, lead veins at, 78 Silver and its ores, 67-69 Andacaba workings, 68 and copper separation, special furnace for, 200 assaying to determine presence of gold, 262-265 black, of Cardano, 53 Caquingora, ores in house walls, 71 Caricari, mines at, 69 cementation method of parting gold and, 270, 271 Chaqui, rich mines of, ¡o Charcas' abundance of, 68 Charcas, Province of, mines in, ¡o Chocaya, rich mines at, 68 Choquepiña, mines at, 67 · comparison with gold, 67 cupelling bottoms for refining, 241243 Encomenderos mine, 71 Guariquari, mines at, 69 La Paz, District of, mines of, ¡o losses thxough carelessness in amalgamating, 94 New Potosí, mines of, 69 ores usually red, 59 Oruro's mines of powdered, 68 Pacajes, Province of, mines of, 70 parting from copper, with recovery of both, 252, 253 parting from gold, warnings, 259-261 parting from gold with nitric acid, 256-258 Piquifa, mines at, 69 properties of, 67 Province of Los Chichas, mines of, 69 refining, warnings in regard to, 246248 separated from gold by use of antimony, 270, 271 Siporo, mines at, 69 1 substances used in dissolving, 2&6 · Tabaco Nuño, mines at, 68
Silver, treating ores of, by amalgamation, 93, 94 Turco, mines at, 67 Vera Cruz, mines at, 69 Yaco, mines at, 68 Yulloma, Indian mines at, 71 Slag, 85 Smell of metals, 53 Smells of the earths, 3-6 Smelter, instruments required by, 203206 Smelting, reduction of all classes of ores by, 185-239 aids in, 2u, 212 "artificialsalt" asa flux, 2II black sulphides, 228 collector for silver ores in, 209, 210 fi.ne-crushing, 207 furnaces, materials from which made, 187 galena ores, charging reverberatories, 226 in Castellano (shaft) furnaces, 229235 iron ore, 236, 23 7 lead as a collector, 2u litharge as a flux, 212 on a bath, sorne warnings, 224, 225 preparing ores for, 207, 2o8 reduction of all classes of ore by, 185239 reverberatory, on a large scale, 222, 223 rich ores require, 185 roasting, 207 shaft furnaces, ores containing gold and silver, 230 copper ores, 232 copper sulphides, 232 heavy lead, 230 lead and copper ores, 230 precautions to be taken in, 234, 235 ruby silver ores, 231 sulphur and antimony ores, 230 sorting previous to, 209 tin ores, 233 use and necessity of, 185, 186 with charcoal, 197, 198 Fll:\DAC IÓN JCANELO TURRIANO
INDEX Solimán (corrosive sui:Ílimate), Sr, S4, 123, 179 "Sombreros (hats, irregular ore deposits), ÓI
Taste, of metals, 53 Theophrastus, exhalations of earth, 2 on sulphur, 23 Thermis, by Andres Baccio Elpidiano1 153 Tiaguanaco, rso Tin, 79, 8o a crying metal, 79 Carabuco, Indian workings, 79 Chayanta district, deposits in, 79 Colquiri district, deposits of, 79 moisture in, 52 origin is same as of lead, 79 plomo blanco (white lead), 79 properties of, 79 San Bernardo parish mines, So Tintin (mortar and pestle) treatment; 182 Tirocinio Chimico, Béguin's, 17 Tocochimbos (muffle furnaces), 194, 198, 200 Tools required by smeltcr, 203-206 Transmutation of metals, 49 artificial, 49, so Trapiche (Chilean mili) metbod of crushing, 1S3 Trinidad Hill, 223, 247 Tumaquifa, 15 boiling lake at, 15 Turco, Province of Carangas, sS, 73, IS2, 195
Soroche (galena), 24; 77, 9S "Spines," 253 Spodium, ss Squeezing and retorting tbe amalgam, 142 Steel-water, 153 Stones, definition ·of, u Albertus, on constituents of, 2S Atacama's many-hued, 37 Avicenna on constituents of, 2S figures of animals, etc., in, 40 genesis of, 2S, 29 humidity and other qualities of, 39 irregularities and their causes, 39-42 precious, 32, 33 indications of in Bolivia, 34 remarkable vari-coloured slab, 3S varieties of, 30, 31 Suco (chloride), 97 Sudnos Mountains, Bohemia, discovery of bismutb in, SS Sulphur, a destroyer of metal, 115 as agent for separating gold and silver, 270, 271 witb mercury a component of metals, 46-4S Sulphur and antimony, 23-25 a case of transmutation, 23 u medicinal value of oil of sulphur, 23 Theophrastus prepares a magic oil illphstadio's Alchemy, 272 from sulphur, 23 de Ureña, Bernardo, royal commissioner, iv, v
Tabaco Nuño, wonderful reservoir at, 6S Tacana (silver sulphide), 96, 9S, 99 Tacora, 24 Tarabuco, 149 copper workings, 73 Tarija, petrifactions at, 29 Tartar emetic, 24 Tarua, copper mint!s at, 73 Taste of earths, 7 moisture the basis of pleasant, 7
V Valaterrano, Rafael, 17 Valentine, Basil, "Triumphal Car of Antimony," 24 fuestone of, 24 Veguino, 24 Veins, ore, classification of, 6r ore, definition of, 6r direction of as governing richness of, 62 mantos (blanket veins), 6r FU:\DACIÓN JCANELO TURRJANO
Veins, varieties of, and how to recognize them, 61-63 signs of richness, 63 Verdigris, 86 Vermicular, 86 Verona, 40 Vilaciques, 31 de Villanova, Amoldo, on conservation of youth, 16 Vitriol an enemy of quicksilver, 101, 106 the basis of metal generation, 44 the source of comets, lightning, etc., 45
Vitriolum (copperas), 13
w Water absorbs qualities of substances by contact, 153, 154
Wet-crushing, altematives to, 183, 184 Wind furnaces (guayras), 198 Wood as fuel in smelting furnaces, 194196
Yanquegua, fire-assay of ore from abandoned mine, 96 Yareta (Bolivian plant used for fuel), 173, 192, 242 Y ellow ochre, 86
Yocalla, salt mines of, 16 Yulloma, 16 copper veins at, 73 stone baptismal font at, 38 Yuyama, 35 Z Zanzibar, 20
FlJ.\DACIĂ“N !CANELO TURRIANO
FLJ:'./DACIÓN JCANELO TURRIANO
Flfl\DACIÓN JCANELO TURR IANO
ll' ~~ J
Fln\'DACIÓN JLAJ'\ELO TURRIANO